# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry A.
# This journal is © The Royal Society of Chemistry 2020

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_sha
_audit_block_doi                 10.5517/ccdc.csd.cc22zk6v
_database_code_depnum_ccdc_archive 'CCDC 1935987'
loop_
_audit_author_name
_audit_author_address
'Jingquan Sha'
; Department of Chemistry and Chemical Engineering, Jining University
China
;
_audit_update_record             
;
2019-06-24 deposited with the CCDC.	2020-11-13 downloaded from the CCDC.
;
_audit_creation_date             2018-11-26
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2014/7
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'C48 Co14 N72 O92 V4 W24, 2(O8 P), 24(O)'
_chemical_formula_sum            'C48 Co14 N72 O132 P2 V4 W24'
_chemical_formula_weight         9200.08
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      tetragonal
_space_group_IT_number           87
_space_group_name_H-M_alt        'I 4/m'
_space_group_name_Hall           '-I 4'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'

_cell_length_a                   17.7970(4)
_cell_length_b                   17.7970(4)
_cell_length_c                   30.1007(13)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     9533.9(6)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    7613
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.299
_cell_measurement_theta_min      2.330
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    15.910
_exptl_absorpt_correction_T_max  0.280
_exptl_absorpt_correction_T_min  0.098
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    3.205
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             8248.0
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.08
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0391
_diffrn_reflns_av_unetI/netI     0.0311
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       39
_diffrn_reflns_limit_l_min       -34
_diffrn_reflns_number            28660
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.520
_diffrn_reflns_theta_min         1.329
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                4527
_reflns_number_total             5615
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v7.68A (Bruker, 2009)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v7.68A (Bruker, 2009)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    ?
_refine_diff_density_max         3.127
_refine_diff_density_min         -6.801
_refine_diff_density_rms         0.451
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.076
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     341
_refine_ls_number_reflns         5610
_refine_ls_number_restraints     14
_refine_ls_R_factor_all          0.0768
_refine_ls_R_factor_gt           0.0607
_refine_ls_restrained_S_all      1.074
_refine_ls_shift/su_max          0.016
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0935P)²+874.5012P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1785
_refine_ls_wR_factor_ref         0.1898
_refine_special_details          ?
_olex2_refinement_description    
;
1. Restrained distances
 O13-P1
 1.5 with sigma of 0.02
 O14-P2
 1.51 with sigma of 0.02
2. Uiso/Uaniso restraints and constraints
Uanis(N3) \\sim Ueq, Uanis(O6W) \\sim Ueq: with sigma of 0.001 and sigma for
terminal atoms of 0.002
3. Others
 Fixed X: P2(0.5)
 Fixed Y: P2(0.5)
 Fixed Z: P2(0.5)
4.a Free rotating group:
 O3W(O4W,O5W,O6W)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.6266(7) 0.3733(7) 0.2382(5) 0.017(3) Uani 1 1 d . . . . .
C2 C 0.5412(7) 0.3405(7) 0.2823(5) 0.016(2) Uani 1 1 d . . . . .
C3 C 0.7075(11) 0.1915(11) 0.3854(6) 0.041(4) Uani 1 1 d . . . . .
C4 C 0.8031(9) 0.2308(9) 0.3473(6) 0.031(3) Uani 1 1 d . . . . .
V2 V 0.5000 0.5000 0.3703(5) 0.100(4) Uani 1 4 d S T P . .
V1 V 0.5000 0.5000 0.1320(5) 0.123(5) Uani 1 4 d S T P . .
C5 C 0.4506(7) 0.1268(7) 0.2493(5) 0.016(2) Uani 1 1 d . . . . .
C6 C 0.7070(7) 0.0953(7) 0.2077(4) 0.015(2) Uani 1 1 d . . . . .
N1 N 0.5914(5) 0.2858(5) 0.2828(4) 0.0111(19) Uani 1 1 d . . . . .
N2 N 0.6471(5) 0.3076(6) 0.2542(4) 0.013(2) Uani 1 1 d . . . . .
N3 N 0.5604(6) 0.3968(6) 0.2540(3) 0.012(2) Uani 1 1 d . U . . .
N4 N 0.6362(6) 0.1197(6) 0.2640(4) 0.015(2) Uani 1 1 d . . . . .
N5 N 0.6898(6) 0.1489(5) 0.2365(4) 0.014(2) Uani 1 1 d . . . . .
N6 N 0.6860(6) 0.1976(6) 0.3447(4) 0.019(2) Uani 1 1 d . . . . .
N7 N 0.7455(6) 0.2253(6) 0.3197(4) 0.017(2) Uani 1 1 d . . . . .
N8 N 0.7812(9) 0.2111(10) 0.3890(5) 0.042(4) Uani 1 1 d . . . . .
O1 O 0.5000 0.5000 0.3196(7) 0.027(4) Uani 1 4 d S T P . .
O2 O 0.5000 0.5000 0.1824(7) 0.023(4) Uani 1 4 d S T P . .
O3 O 0.3977(6) 0.6645(9) 0.4570(5) 0.055(5) Uani 1 1 d . . . . .
O4 O 0.3307(7) 0.6234(8) 0.3781(4) 0.040(3) Uani 1 1 d . . . . .
O5 O 0.2085(9) 0.4533(9) 0.5000 0.042(5) Uani 1 2 d S T P . .
O6 O 0.4208(8) 0.5635(7) 0.1050(5) 0.054(4) Uani 1 1 d . . . . .
O7 O 0.2923(6) 0.4756(8) 0.1226(4) 0.039(3) Uani 1 1 d . . . . .
Co1 Co 0.57868(9) 0.18029(9) 0.31308(5) 0.0095(3) Uani 1 1 d . . . . .
Co3 Co 0.5000 0.5000 0.25003(10) 0.0066(6) Uani 1 4 d S T P . .
W1 W 0.35759(4) 0.48450(4) 0.08246(2) 0.02740(19) Uani 1 1 d . . . . .
W2 W 0.30146(5) 0.46690(5) 0.5000 0.0293(2) Uani 1 2 d S T P . .
W3 W 0.38396(4) 0.58453(4) 0.41819(2) 0.02938(19) Uani 1 1 d . . . . .
W4 W 0.37739(6) 0.34307(6) 0.0000 0.0397(3) Uani 1 2 d S T P . .
P2 P 0.5000 0.5000 0.5000 0.0053(14) Uani 1 8 d DS T P . .
P1 P 0.5000 0.5000 0.0000 0.0062(14) Uani 1 8 d DS T P . .
Co2 Co 0.7500 0.2500 0.2500 0.0094(4) Uani 1 2 d S T P . .
N9 N 0.4695(6) 0.1687(6) 0.2845(4) 0.014(2) Uani 1 1 d . . . . .
O8 O 0.3118(9) 0.5445(7) 0.4566(5) 0.057(5) Uani 1 1 d . . . . .
O9 O 0.3290(8) 0.4039(9) 0.0452(5) 0.054(4) Uani 1 1 d . . . . .
O10 O 0.3140(9) 0.5506(8) 0.0436(5) 0.063(5) Uani 1 1 d . . . . .
O11 O 0.2696(10) 0.6801(10) 0.0000 0.045(5) Uani 1 2 d S T P . .
O12 O 0.3983(8) 0.4829(6) 0.3945(5) 0.044(4) Uani 1 1 d . . . . .
O13 O 0.4451(8) 0.5421(9) 0.0292(5) 0.058(4) Uani 1 1 d D . . . .
O1W O 0.5596(7) 0.0764(6) 0.3488(4) 0.038(3) Uani 1 1 d . . . . .
O2W O 0.5289(6) 0.2298(7) 0.3710(4) 0.034(3) Uani 1 1 d . . . . .
O3W O 0.6481(12) -0.0457(11) 0.3453(9) 0.134(12) Uani 1 1 d . . . . .
O4W O 0.2821(17) 0.8369(13) 0.0001(15) 0.123(15) Uani 1 2 d GS T P . .
O5W O 0.4102(13) 0.1507(13) 0.4118(9) 0.157(15) Uani 1 1 d G . . . .
O6W O 0.1764(18) 0.4762(14) 0.0000(13) 0.160(18) Uani 1 2 d GS TU P . .
O14 O 0.5696(8) 0.5103(9) 0.5283(5) 0.055(4) Uiso 1 1 d D . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
C1 N2 1.317(16) . ?
C1 N3 1.336(15) . ?
C2 N1 1.322(15) . ?
C2 N3 1.357(16) . ?
C3 N6 1.29(2) . ?
C3 N8 1.36(2) . ?
C4 N7 1.322(18) . ?
C4 N8 1.36(2) . ?
V2 O1 1.52(2) . ?
V2 W3 2.934(7) 2_665 ?
V2 W3 2.934(7) . ?
V2 W3 2.934(7) 4_565 ?
V2 W3 2.934(7) 3_655 ?
V2 O12 1.975(13) 3_655 ?
V2 O12 1.975(13) 4_565 ?
V2 O12 1.975(13) . ?
V2 O12 1.975(13) 2_665 ?
V1 O2 1.52(3) . ?
V1 O6 1.980(14) 3_655 ?
V1 O6 1.980(14) 2_665 ?
V1 O6 1.980(14) . ?
V1 O6 1.980(14) 4_565 ?
V1 W1 2.954(8) . ?
V1 W1 2.954(8) 4_565 ?
V1 W1 2.954(8) 2_665 ?
V1 W1 2.954(8) 3_655 ?
C5 N4 1.324(15) 16_545 ?
C5 N9 1.338(17) . ?
C6 N5 1.325(16) . ?
C6 N9 1.359(16) 15 ?
N1 N2 1.369(14) . ?
N1 Co1 2.099(10) . ?
N2 Co2 2.102(10) . ?
N3 Co3 2.132(10) . ?
N4 C5 1.324(15) 15 ?
N4 N5 1.367(15) . ?
N4 Co1 2.095(11) . ?
N5 Co2 2.134(10) . ?
N6 N7 1.388(16) . ?
N6 Co1 2.156(11) . ?
N7 Co2 2.147(12) . ?
O1 Co3 2.09(2) . ?
O2 Co3 2.03(2) . ?
O3 W2 1.887(12) 11_566 ?
O3 W3 1.857(12) . ?
O4 W3 1.684(11) . ?
O5 W2 1.673(16) . ?
O6 W1 1.924(12) . ?
O6 W1 1.928(12) 4_565 ?
O7 W1 1.684(11) . ?
Co1 N9 2.136(10) . ?
Co1 O1W 2.165(11) . ?
Co1 O2W 2.146(11) . ?
Co3 N3 2.132(10) 4_565 ?
Co3 N3 2.132(10) 3_655 ?
Co3 N3 2.132(10) 2_665 ?
W1 O6 1.928(12) 3_655 ?
W1 O9 1.892(12) . ?
W1 O10 1.831(13) . ?
W1 O13 2.458(15) . ?
W1 O13 2.499(15) 3_655 ?
W2 O3 1.887(12) 3_655 ?
W2 O3 1.887(12) 12_656 ?
W2 O8 1.909(12) 10_556 ?
W2 O8 1.909(12) . ?
W2 O14 2.481(15) 2_665 ?
W2 O14 2.481(15) 9_666 ?
W3 O8 1.869(12) . ?
W3 O12 1.924(11) 4_565 ?
W3 O12 1.961(11) . ?
W3 O14 2.474(15) 9_666 ?
W3 O14 2.491(15) 12_656 ?
W4 O9 1.939(12) 10 ?
W4 O9 1.939(12) . ?
W4 O10 1.906(12) 12_655 ?
W4 O10 1.906(12) 3_655 ?
W4 O11 1.661(18) 3_655 ?
W4 O13 2.475(15) 3_655 ?
W4 O13 2.475(15) 12_655 ?
P2 O14 1.515(13) . ?
P2 O14 1.515(13) 11_566 ?
P2 O14 1.515(13) 3_655 ?
P2 O14 1.515(13) 10_556 ?
P2 O14 1.515(13) 12_656 ?
P2 O14 1.515(13) 4_565 ?
P2 O14 1.515(13) 2_665 ?
P2 O14 1.515(13) 9_666 ?
P1 O13 1.513(13) . ?
P1 O13 1.513(13) 11_565 ?
P1 O13 1.513(13) 3_655 ?
P1 O13 1.513(13) 10 ?
P1 O13 1.513(13) 2_665 ?
P1 O13 1.513(13) 9_665 ?
P1 O13 1.513(13) 12_655 ?
P1 O13 1.513(13) 4_565 ?
Co2 N2 2.102(10) 13_655 ?
Co2 N5 2.134(10) 13_655 ?
Co2 N7 2.146(12) 13_655 ?
N9 C6 1.359(16) 16_545 ?
O10 W4 1.906(12) 11_565 ?
O11 W4 1.661(18) 11_565 ?
O12 W3 1.924(11) 3_655 ?
O13 W1 2.499(15) 4_565 ?
O13 W4 2.475(15) 11_565 ?
O14 W2 2.481(15) 9_666 ?
O14 W3 2.491(15) 11_566 ?
O14 W3 2.474(15) 9_666 ?
O14 O14 1.71(3) 10_556 ?
O14 O14 1.771(19) 3_655 ?
O14 O14 1.771(19) 4_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N2 C1 N3 113.1(11) . . ?
N1 C2 N3 112.4(11) . . ?
N6 C3 N8 110.0(16) . . ?
N7 C4 N8 109.8(14) . . ?
O1 V2 W3 119.4(2) . 4_565 ?
O1 V2 W3 119.4(2) . . ?
O1 V2 W3 119.4(2) . 3_655 ?
O1 V2 W3 119.4(2) . 2_665 ?
O1 V2 O12 111.7(6) . . ?
O1 V2 O12 111.7(6) . 4_565 ?
O1 V2 O12 111.7(6) . 3_655 ?
O1 V2 O12 111.7(6) . 2_665 ?
W3 V2 W3 76.0(2) 3_655 2_665 ?
W3 V2 W3 76.0(2) 4_565 2_665 ?
W3 V2 W3 76.0(2) . 4_565 ?
W3 V2 W3 76.0(2) . 3_655 ?
W3 V2 W3 121.1(5) 4_565 3_655 ?
W3 V2 W3 121.1(5) . 2_665 ?
O12 V2 W3 113.4(6) 3_655 . ?
O12 V2 W3 40.5(3) . 3_655 ?
O12 V2 W3 113.4(6) 2_665 3_655 ?
O12 V2 W3 41.6(4) 2_665 2_665 ?
O12 V2 W3 40.5(3) 2_665 4_565 ?
O12 V2 W3 40.5(3) 4_565 . ?
O12 V2 W3 41.6(4) 4_565 4_565 ?
O12 V2 W3 40.5(3) 3_655 2_665 ?
O12 V2 W3 112.6(6) . 2_665 ?
O12 V2 W3 112.6(6) 2_665 . ?
O12 V2 W3 112.6(6) 3_655 4_565 ?
O12 V2 W3 113.4(6) . 4_565 ?
O12 V2 W3 112.6(6) 4_565 3_655 ?
O12 V2 W3 41.6(4) 3_655 3_655 ?
O12 V2 W3 113.4(6) 4_565 2_665 ?
O12 V2 W3 41.6(4) . . ?
O12 V2 O12 82.2(4) 2_665 3_655 ?
O12 V2 O12 136.7(12) 2_665 . ?
O12 V2 O12 136.7(12) 4_565 3_655 ?
O12 V2 O12 82.2(4) 4_565 . ?
O12 V2 O12 82.2(4) 3_655 . ?
O12 V2 O12 82.2(4) 2_665 4_565 ?
O2 V1 O6 114.2(7) . 3_655 ?
O2 V1 O6 114.2(7) . 2_665 ?
O2 V1 O6 114.2(7) . . ?
O2 V1 O6 114.2(7) . 4_565 ?
O2 V1 W1 120.3(3) . . ?
O2 V1 W1 120.3(3) . 4_565 ?
O2 V1 W1 120.3(3) . 2_665 ?
O2 V1 W1 120.3(3) . 3_655 ?
O6 V1 O6 80.3(5) 3_655 2_665 ?
O6 V1 O6 80.3(5) 3_655 . ?
O6 V1 O6 131.5(13) 2_665 . ?
O6 V1 O6 131.5(13) 3_655 4_565 ?
O6 V1 O6 80.3(5) 4_565 . ?
O6 V1 O6 80.3(5) 4_565 2_665 ?
O6 V1 W1 110.5(7) . 2_665 ?
O6 V1 W1 110.4(7) 2_665 4_565 ?
O6 V1 W1 110.5(7) 3_655 4_565 ?
O6 V1 W1 110.5(7) 4_565 3_655 ?
O6 V1 W1 40.3(4) 4_565 2_665 ?
O6 V1 W1 40.3(4) . 4_565 ?
O6 V1 W1 40.1(4) . . ?
O6 V1 W1 40.1(4) 4_565 4_565 ?
O6 V1 W1 40.1(4) 2_665 2_665 ?
O6 V1 W1 110.4(7) . 3_655 ?
O6 V1 W1 110.5(7) 2_665 . ?
O6 V1 W1 40.3(4) 3_655 . ?
O6 V1 W1 40.1(4) 3_655 3_655 ?
O6 V1 W1 110.4(7) 4_565 . ?
O6 V1 W1 40.3(4) 2_665 3_655 ?
O6 V1 W1 110.4(7) 3_655 2_665 ?
W1 V1 W1 75.2(2) . 4_565 ?
W1 V1 W1 119.3(5) . 2_665 ?
W1 V1 W1 75.2(2) . 3_655 ?
W1 V1 W1 75.2(2) 4_565 2_665 ?
W1 V1 W1 75.2(2) 3_655 2_665 ?
W1 V1 W1 119.3(5) 3_655 4_565 ?
N4 C5 N9 114.0(11) 16_545 . ?
N5 C6 N9 112.4(11) . 15 ?
C2 N1 N2 105.9(10) . . ?
C2 N1 Co1 126.3(8) . . ?
N2 N1 Co1 127.2(7) . . ?
C1 N2 N1 106.3(9) . . ?
C1 N2 Co2 130.8(8) . . ?
N1 N2 Co2 122.1(7) . . ?
C1 N3 C2 102.4(10) . . ?
C1 N3 Co3 133.9(9) . . ?
C2 N3 Co3 122.9(8) . . ?
C5 N4 N5 105.2(11) 15 . ?
C5 N4 Co1 129.7(9) 15 . ?
N5 N4 Co1 125.0(8) . . ?
C6 N5 N4 106.5(10) . . ?
C6 N5 Co2 128.1(9) . . ?
N4 N5 Co2 123.7(8) . . ?
C3 N6 N7 108.5(13) . . ?
C3 N6 Co1 132.1(12) . . ?
N7 N6 Co1 119.2(8) . . ?
C4 N7 N6 106.2(12) . . ?
C4 N7 Co2 124.7(11) . . ?
N6 N7 Co2 129.0(8) . . ?
C3 N8 C4 105.4(13) . . ?
V2 O1 Co3 180.0 . . ?
V1 O2 Co3 180.0 . . ?
W3 O3 W2 139.8(8) . 11_566 ?
W1 O6 V1 98.2(6) 4_565 . ?
W1 O6 V1 98.3(6) . . ?
W1 O6 W1 138.8(9) . 4_565 ?
N1 Co1 N6 88.2(4) . . ?
N1 Co1 N9 90.5(4) . . ?
N1 Co1 O1W 174.9(4) . . ?
N1 Co1 O2W 91.8(5) . . ?
N4 Co1 N1 95.8(4) . . ?
N4 Co1 N6 87.2(4) . . ?
N4 Co1 N9 96.3(4) . . ?
N4 Co1 O1W 89.2(4) . . ?
N4 Co1 O2W 170.4(5) . . ?
N6 Co1 O1W 92.4(5) . . ?
N9 Co1 N6 176.3(4) . . ?
N9 Co1 O1W 88.6(5) . . ?
N9 Co1 O2W 89.5(4) . . ?
O2W Co1 N6 87.1(5) . . ?
O2W Co1 O1W 83.3(5) . . ?
N3 Co3 N3 173.6(6) . 2_665 ?
N3 Co3 N3 89.82(3) 3_655 2_665 ?
N3 Co3 N3 173.6(6) 3_655 4_565 ?
N3 Co3 N3 89.82(3) 4_565 2_665 ?
N3 Co3 N3 89.82(3) . 3_655 ?
N3 Co3 N3 89.82(3) . 4_565 ?
O1 Co3 N3 86.8(3) . 2_665 ?
O1 Co3 N3 86.8(3) . 4_565 ?
O1 Co3 N3 86.8(3) . . ?
O1 Co3 N3 86.8(3) . 3_655 ?
O2 Co3 N3 93.2(3) . 4_565 ?
O2 Co3 N3 93.2(3) . 2_665 ?
O2 Co3 N3 93.2(3) . 3_655 ?
O2 Co3 N3 93.2(3) . . ?
O2 Co3 O1 180.0 . . ?
O6 W1 V1 41.6(4) . . ?
O6 W1 V1 41.6(4) 3_655 . ?
O6 W1 O6 83.0(8) . 3_655 ?
O6 W1 O13 90.7(7) 3_655 . ?
O6 W1 O13 62.6(6) 3_655 3_655 ?
O6 W1 O13 63.6(6) . . ?
O6 W1 O13 90.7(7) . 3_655 ?
O7 W1 V1 103.8(5) . . ?
O7 W1 O6 101.2(7) . 3_655 ?
O7 W1 O6 102.7(7) . . ?
O7 W1 O9 99.7(7) . . ?
O7 W1 O10 103.1(7) . . ?
O7 W1 O13 160.8(6) . . ?
O7 W1 O13 157.9(6) . 3_655 ?
O9 W1 V1 127.0(4) . . ?
O9 W1 O6 87.7(5) . 3_655 ?
O9 W1 O6 157.0(7) . . ?
O9 W1 O13 66.4(6) . 3_655 ?
O9 W1 O13 95.7(6) . . ?
O10 W1 V1 128.7(4) . . ?
O10 W1 O6 90.2(5) . . ?
O10 W1 O6 155.6(8) . 3_655 ?
O10 W1 O9 89.7(6) . . ?
O10 W1 O13 94.2(7) . 3_655 ?
O10 W1 O13 65.4(6) . . ?
O13 W1 V1 75.3(4) . . ?
O13 W1 V1 74.7(4) 3_655 . ?
O13 W1 O13 41.1(6) . 3_655 ?
O3 W2 O3 86.6(9) 3_655 12_656 ?
O3 W2 O8 88.4(5) 12_656 10_556 ?
O3 W2 O8 155.5(8) 3_655 10_556 ?
O3 W2 O8 88.4(5) 3_655 . ?
O3 W2 O8 155.5(8) 12_656 . ?
O3 W2 O14 92.6(7) 12_656 9_666 ?
O3 W2 O14 92.6(7) 3_655 2_665 ?
O3 W2 O14 64.8(6) 12_656 2_665 ?
O3 W2 O14 64.8(6) 3_655 9_666 ?
O5 W2 O3 102.9(7) . 12_656 ?
O5 W2 O3 102.9(7) . 3_655 ?
O5 W2 O8 101.6(7) . . ?
O5 W2 O8 101.6(7) . 10_556 ?
O5 W2 O14 159.8(3) . 9_666 ?
O5 W2 O14 159.8(3) . 2_665 ?
O8 W2 O8 86.3(9) 10_556 . ?
O8 W2 O14 91.6(7) . 2_665 ?
O8 W2 O14 63.7(6) 10_556 2_665 ?
O8 W2 O14 91.6(7) 10_556 9_666 ?
O8 W2 O14 63.7(6) . 9_666 ?
O14 W2 O14 40.2(6) 2_665 9_666 ?
O3 W3 V2 127.5(4) . . ?
O3 W3 O8 89.6(6) . . ?
O3 W3 O12 156.7(7) . . ?
O3 W3 O12 89.5(5) . 4_565 ?
O3 W3 O14 94.0(7) . 9_666 ?
O3 W3 O14 64.9(6) . 12_656 ?
O4 W3 V2 104.8(5) . . ?
O4 W3 O3 102.2(7) . . ?
O4 W3 O8 102.3(7) . . ?
O4 W3 O12 101.0(7) . . ?
O4 W3 O12 100.6(7) . 4_565 ?
O4 W3 O14 159.2(6) . 9_666 ?
O4 W3 O14 158.9(6) . 12_656 ?
O8 W3 V2 126.3(4) . . ?
O8 W3 O12 156.7(7) . 4_565 ?
O8 W3 O12 87.9(5) . . ?
O8 W3 O14 94.5(7) . 12_656 ?
O8 W3 O14 64.3(6) . 9_666 ?
O12 W3 V2 42.0(4) . . ?
O12 W3 V2 41.9(4) 4_565 . ?
O12 W3 O12 83.9(7) 4_565 . ?
O12 W3 O14 92.2(6) . 12_656 ?
O12 W3 O14 64.2(6) 4_565 12_656 ?
O12 W3 O14 92.5(6) 4_565 9_666 ?
O12 W3 O14 64.2(5) . 9_666 ?
O14 W3 V2 74.6(4) 9_666 . ?
O14 W3 V2 74.4(4) 12_656 . ?
O14 W3 O14 41.8(5) 9_666 12_656 ?
O9 W4 O9 89.0(8) . 10 ?
O9 W4 O13 95.6(6) . 12_655 ?
O9 W4 O13 66.3(6) 10 12_655 ?
O9 W4 O13 95.6(6) 10 3_655 ?
O9 W4 O13 66.3(6) . 3_655 ?
O10 W4 O9 88.1(5) 3_655 . ?
O10 W4 O9 158.9(8) 12_655 . ?
O10 W4 O9 88.1(5) 12_655 10 ?
O10 W4 O9 158.9(8) 3_655 10 ?
O10 W4 O10 87.1(9) 3_655 12_655 ?
O10 W4 O13 64.2(6) 12_655 12_655 ?
O10 W4 O13 93.1(7) 12_655 3_655 ?
O10 W4 O13 93.1(7) 3_655 12_655 ?
O10 W4 O13 64.2(6) 3_655 3_655 ?
O11 W4 O9 99.6(7) 3_655 . ?
O11 W4 O9 99.6(7) 3_655 10 ?
O11 W4 O10 101.6(7) 3_655 3_655 ?
O11 W4 O10 101.6(7) 3_655 12_655 ?
O11 W4 O13 159.2(3) 3_655 3_655 ?
O11 W4 O13 159.2(3) 3_655 12_655 ?
O13 W4 O13 41.6(6) 3_655 12_655 ?
O14 P2 O14 108.5(6) . 12_656 ?
O14 P2 O14 71.5(6) 9_666 11_566 ?
O14 P2 O14 108.5(6) 10_556 4_565 ?
O14 P2 O14 71.5(6) 9_666 12_656 ?
O14 P2 O14 71.5(6) . 3_655 ?
O14 P2 O14 111.5(12) 11_566 12_656 ?
O14 P2 O14 180.0(9) 11_566 3_655 ?
O14 P2 O14 180.0(9) 12_656 4_565 ?
O14 P2 O14 180.0 . 9_666 ?
O14 P2 O14 108.5(6) 9_666 3_655 ?
O14 P2 O14 108.5(6) 3_655 10_556 ?
O14 P2 O14 111.5(12) 3_655 4_565 ?
O14 P2 O14 111.5(12) . 2_665 ?
O14 P2 O14 180.0 10_556 2_665 ?
O14 P2 O14 108.5(6) 11_566 2_665 ?
O14 P2 O14 108.5(6) 9_666 4_565 ?
O14 P2 O14 108.5(6) 12_656 2_665 ?
O14 P2 O14 68.5(12) 9_666 2_665 ?
O14 P2 O14 71.5(6) . 4_565 ?
O14 P2 O14 71.5(6) 3_655 2_665 ?
O14 P2 O14 68.5(12) 11_566 4_565 ?
O14 P2 O14 71.5(6) 11_566 10_556 ?
O14 P2 O14 68.5(12) . 10_556 ?
O14 P2 O14 71.5(6) 12_656 10_556 ?
O14 P2 O14 111.5(12) 9_666 10_556 ?
O14 P2 O14 108.5(6) . 11_566 ?
O14 P2 O14 71.5(6) 2_665 4_565 ?
O14 P2 O14 68.5(12) 3_655 12_656 ?
O13 P1 O13 109.8(6) . 12_655 ?
O13 P1 O13 109.8(6) 2_665 11_565 ?
O13 P1 O13 108.9(11) 4_565 3_655 ?
O13 P1 O13 108.9(11) 12_655 11_565 ?
O13 P1 O13 70.2(6) . 3_655 ?
O13 P1 O13 108.9(11) 10 9_665 ?
O13 P1 O13 109.8(6) . 11_565 ?
O13 P1 O13 70.2(6) . 4_565 ?
O13 P1 O13 180.0(12) 3_655 11_565 ?
O13 P1 O13 180.0 . 9_665 ?
O13 P1 O13 71.1(11) 12_655 3_655 ?
O13 P1 O13 180.0(12) 12_655 4_565 ?
O13 P1 O13 71.1(11) 4_565 11_565 ?
O13 P1 O13 109.8(6) 10 3_655 ?
O13 P1 O13 70.2(6) 12_655 10 ?
O13 P1 O13 108.9(11) . 2_665 ?
O13 P1 O13 109.8(6) 4_565 10 ?
O13 P1 O13 70.2(6) 10 11_565 ?
O13 P1 O13 180.0(9) 2_665 10 ?
O13 P1 O13 109.8(6) 12_655 2_665 ?
O13 P1 O13 71.1(11) 2_665 9_665 ?
O13 P1 O13 109.8(6) 4_565 9_665 ?
O13 P1 O13 109.8(6) 3_655 9_665 ?
O13 P1 O13 70.2(6) 4_565 2_665 ?
O13 P1 O13 70.2(6) 2_665 3_655 ?
O13 P1 O13 70.2(6) 11_565 9_665 ?
O13 P1 O13 71.1(11) . 10 ?
O13 P1 O13 70.2(6) 12_655 9_665 ?
N2 Co2 N2 180.0 . 13_655 ?
N2 Co2 N5 89.2(4) 13_655 13_655 ?
N2 Co2 N5 90.8(4) . 13_655 ?
N2 Co2 N5 90.8(4) 13_655 . ?
N2 Co2 N5 89.2(4) . . ?
N2 Co2 N7 89.5(4) . 13_655 ?
N2 Co2 N7 89.5(4) 13_655 . ?
N2 Co2 N7 90.5(4) 13_655 13_655 ?
N2 Co2 N7 90.5(4) . . ?
N5 Co2 N5 180.0 . 13_655 ?
N5 Co2 N7 90.3(4) . 13_655 ?
N5 Co2 N7 89.7(4) . . ?
N5 Co2 N7 90.3(4) 13_655 . ?
N5 Co2 N7 89.7(4) 13_655 13_655 ?
N7 Co2 N7 180.0(5) 13_655 . ?
C5 N9 C6 101.8(10) . 16_545 ?
C5 N9 Co1 127.0(8) . . ?
C6 N9 Co1 130.7(9) 16_545 . ?
W3 O8 W2 139.9(9) . . ?
W1 O9 W4 136.0(9) . . ?
W1 O10 W4 139.2(10) . 11_565 ?
W3 O12 V2 97.6(6) 3_655 . ?
W3 O12 V2 96.4(6) . . ?
W3 O12 W3 136.9(8) 3_655 . ?
W1 O13 W1 93.3(5) . 4_565 ?
W1 O13 W4 90.5(5) . 11_565 ?
W4 O13 W1 91.1(5) 11_565 4_565 ?
P1 O13 W1 125.6(9) . . ?
P1 O13 W1 123.0(8) . 4_565 ?
P1 O13 W4 123.6(8) . 11_565 ?
W3 O14 W2 90.0(5) 11_566 9_666 ?
W3 O14 W2 91.5(5) 9_666 9_666 ?
W3 O14 W3 93.4(5) 9_666 11_566 ?
P2 O14 W2 125.6(8) . 9_666 ?
P2 O14 W3 122.8(8) . 11_566 ?
P2 O14 W3 123.8(8) . 9_666 ?
P2 O14 O14 54.2(3) . 4_565 ?
P2 O14 O14 54.2(3) . 3_655 ?
P2 O14 O14 55.7(6) . 10_556 ?
O14 O14 W2 69.9(3) 10_556 9_666 ?
O14 O14 W2 133.0(10) 4_565 9_666 ?
O14 O14 W2 130.2(10) 3_655 9_666 ?
O14 O14 W3 130.3(4) 10_556 11_566 ?
O14 O14 W3 132.4(4) 3_655 9_666 ?
O14 O14 W3 132.1(4) 4_565 11_566 ?
O14 O14 W3 130.6(4) 10_556 9_666 ?
O14 O14 W3 68.6(7) 3_655 11_566 ?
O14 O14 W3 69.6(7) 4_565 9_666 ?
O14 O14 O14 90.005(2) 10_556 3_655 ?
O14 O14 O14 90.004(5) 10_556 4_565 ?
O14 O14 O14 90.002(4) 3_655 4_565 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
C2 N1 N2 C1 -0.6(14) . . . . ?
C2 N1 N2 Co2 169.7(9) . . . . ?
C3 N6 N7 C4 3.4(17) . . . . ?
C3 N6 N7 Co2 -179.6(12) . . . . ?
V2 W3 O8 W2 36.0(18) . . . . ?
V1 W1 O9 W4 -42.6(15) . . . . ?
V1 W1 O10 W4 34.3(19) . . . 11_565 ?
C5 N4 N5 C6 2.1(14) 15 . . . ?
C5 N4 N5 Co2 -164.1(9) 15 . . . ?
N1 C2 N3 C1 -1.6(15) . . . . ?
N1 C2 N3 Co3 -172.6(8) . . . . ?
N2 C1 N3 C2 1.2(15) . . . . ?
N2 C1 N3 Co3 170.7(9) . . . . ?
N3 C1 N2 N1 -0.4(15) . . . . ?
N3 C1 N2 Co2 -169.5(9) . . . . ?
N3 C2 N1 N2 1.4(15) . . . . ?
N3 C2 N1 Co1 -169.7(8) . . . . ?
N4 C5 N9 C6 -0.8(15) 16_545 . . 16_545 ?
N4 C5 N9 Co1 -173.4(9) 16_545 . . . ?
N6 C3 N8 C4 1(2) . . . . ?
N7 C4 N8 C3 1(2) . . . . ?
N8 C3 N6 N7 -3(2) . . . . ?
N8 C3 N6 Co1 -177.9(12) . . . . ?
N8 C4 N7 N6 -2.9(18) . . . . ?
N8 C4 N7 Co2 180.0(11) . . . . ?
O3 W3 O8 W2 -102.7(15) . . . . ?
O4 W3 O8 W2 154.9(14) . . . . ?
O6 W1 O9 W4 -57.2(12) 3_655 . . . ?
O6 W1 O9 W4 9(2) . . . . ?
O6 W1 O10 W4 51.3(15) . . . 11_565 ?
O6 W1 O10 W4 -22(3) 3_655 . . 11_565 ?
O7 W1 O9 W4 -158.2(12) . . . . ?
O7 W1 O10 W4 154.3(14) . . . 11_565 ?
Co1 N1 N2 C1 170.4(9) . . . . ?
Co1 N1 N2 Co2 -19.3(14) . . . . ?
Co1 N4 N5 C6 -174.0(9) . . . . ?
Co1 N4 N5 Co2 19.7(14) . . . . ?
Co1 N6 N7 C4 179.4(10) . . . . ?
Co1 N6 N7 Co2 -3.6(14) . . . . ?
W2 O3 W3 V2 -34.3(18) 11_566 . . . ?
W2 O3 W3 O4 -153.9(14) 11_566 . . . ?
W2 O3 W3 O8 103.6(15) 11_566 . . . ?
W2 O3 W3 O12 -53.1(14) 11_566 . . 4_565 ?
W2 O3 W3 O12 20(2) 11_566 . . . ?
W2 O3 W3 O14 39.4(14) 11_566 . . 9_666 ?
W2 O3 W3 O14 8.4(12) 11_566 . . 12_656 ?
N9 C6 N5 N4 -1.8(15) 15 . . . ?
N9 C6 N5 Co2 163.7(9) 15 . . . ?
O9 W1 O10 W4 -105.8(15) . . . 11_565 ?
O10 W1 O9 W4 98.6(13) . . . . ?
O12 W3 O8 W2 54.1(14) . . . . ?
O12 W3 O8 W2 -15(3) 4_565 . . . ?
O13 W1 O9 W4 33.3(12) . . . . ?
O13 W1 O9 W4 3.8(10) 3_655 . . . ?
O13 W1 O10 W4 -39.5(15) 3_655 . . 11_565 ?
O13 W1 O10 W4 -9.3(13) . . . 11_565 ?
O13 P1 O13 W1 121.5(3) 3_655 . . 4_565 ?
O13 P1 O13 W1 -118.4(7) 10 . . 4_565 ?
O13 P1 O13 W1 1.8(10) 4_565 . . 4_565 ?
O13 P1 O13 W1 61.6(7) 2_665 . . 4_565 ?
O13 P1 O13 W1 -121.5(4) 4_565 . . . ?
O13 P1 O13 W1 -178.2(10) 12_655 . . 4_565 ?
O13 P1 O13 W1 -1.9(11) 3_655 . . . ?
O13 P1 O13 W1 -61.7(7) 2_665 . . . ?
O13 P1 O13 W1 -58.5(3) 11_565 . . 4_565 ?
O13 P1 O13 W1 58.5(4) 12_655 . . . ?
O13 P1 O13 W1 118.3(7) 10 . . . ?
O13 P1 O13 W1 178.1(11) 11_565 . . . ?
O13 P1 O13 W4 179.1(13) 2_665 . . 11_565 ?
O13 P1 O13 W4 58.9(13) 11_565 . . 11_565 ?
O13 P1 O13 W4 -121.1(13) 3_655 . . 11_565 ?
O13 P1 O13 W4 119.3(13) 4_565 . . 11_565 ?
O13 P1 O13 W4 -60.7(13) 12_655 . . 11_565 ?
O13 P1 O13 W4 -0.9(13) 10 . . 11_565 ?
O14 W3 O8 W2 -37.9(14) 12_656 . . . ?
O14 W3 O8 W2 -8.1(12) 9_666 . . . ?
O14 P2 O14 W2 -178.1(13) 2_665 . . 9_666 ?
O14 P2 O14 W2 -58.8(13) 12_656 . . 9_666 ?
O14 P2 O14 W2 121.2(13) 4_565 . . 9_666 ?
O14 P2 O14 W2 62.5(13) 11_566 . . 9_666 ?
O14 P2 O14 W2 1.9(13) 10_556 . . 9_666 ?
O14 P2 O14 W2 -117.5(13) 3_655 . . 9_666 ?
O14 P2 O14 W3 0.0(11) 4_565 . . 9_666 ?
O14 P2 O14 W3 58.8(3) 12_656 . . 11_566 ?
O14 P2 O14 W3 -121.2(3) 4_565 . . 11_566 ?
O14 P2 O14 W3 -180.0(11) 11_566 . . 11_566 ?
O14 P2 O14 W3 119.4(7) 10_556 . . 11_566 ?
O14 P2 O14 W3 -58.8(4) 11_566 . . 9_666 ?
O14 P2 O14 W3 180.0(11) 12_656 . . 9_666 ?
O14 P2 O14 W3 -60.6(7) 2_665 . . 11_566 ?
O14 P2 O14 W3 0.0(11) 3_655 . . 11_566 ?
O14 P2 O14 W3 121.2(4) 3_655 . . 9_666 ?
O14 P2 O14 W3 60.6(7) 2_665 . . 9_666 ?
O14 P2 O14 W3 -119.4(7) 10_556 . . 9_666 ?
O14 P2 O14 O14 180.000(2) 2_665 . . 10_556 ?
O14 P2 O14 O14 180.000(2) 12_656 . . 4_565 ?
O14 P2 O14 O14 -119.4(4) 3_655 . . 10_556 ?
O14 P2 O14 O14 121.3(7) 3_655 . . 4_565 ?
O14 P2 O14 O14 60.6(4) 2_665 . . 4_565 ?
O14 P2 O14 O14 60.6(4) 11_566 . . 10_556 ?
O14 P2 O14 O14 -58.7(7) 11_566 . . 4_565 ?
O14 P2 O14 O14 119.4(4) 4_565 . . 10_556 ?
O14 P2 O14 O14 119.4(4) 10_556 . . 3_655 ?
O14 P2 O14 O14 -119.4(4) 10_556 . . 4_565 ?
O14 P2 O14 O14 -60.6(4) 2_665 . . 3_655 ?
O14 P2 O14 O14 180.000(2) 11_566 . . 3_655 ?
O14 P2 O14 O14 -121.3(7) 4_565 . . 3_655 ?
O14 P2 O14 O14 -60.6(4) 12_656 . . 10_556 ?
O14 P2 O14 O14 58.7(7) 12_656 . . 3_655 ?


_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_sha_CCDC1
_audit_block_doi                 10.5517/ccdc.csd.cc210br5
_database_code_depnum_ccdc_archive 'CCDC 1877166'
loop_
_audit_author_name
_audit_author_address
'Jingquan Sha'
;Department of Chemistry and Chemical Engineering, Jining University, Qufu, Shandong, 273155, P.R Chi
China
;
_audit_update_record             
;
2018-11-05 deposited with the CCDC.	2020-11-13 downloaded from the CCDC.
;
_audit_creation_date             2018-10-18
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2014/7
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'C24 H40 Co7 Mo12 N36 O54 P V2'
_chemical_formula_sum            'C24 H40 Co7 Mo12 N36 O54 P V2'
_chemical_formula_weight         3393.56
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_H-M_alt        'C 1 2/m 1'
_space_group_name_Hall           '-C 2y'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'

_cell_length_a                   25.151(7)
_cell_length_b                   30.596(12)
_cell_length_c                   17.790(5)
_cell_angle_alpha                90
_cell_angle_beta                 134.947(5)
_cell_angle_gamma                90
_cell_volume                     9689(5)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    28021
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      24.999
_cell_measurement_theta_min      1.323
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    2.958
_exptl_absorpt_correction_T_max  0.837
_exptl_absorpt_correction_T_min  0.572
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    2.326
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             6488.0
_exptl_crystal_size_max          0.21
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.06
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0430
_diffrn_reflns_av_unetI/netI     0.0417
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -29
_diffrn_reflns_limit_k_max       36
_diffrn_reflns_limit_k_min       -35
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            28021
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        24.999
_diffrn_reflns_theta_max         24.999
_diffrn_reflns_theta_min         1.323
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker APEX2 CCD area-detector'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                7637
_reflns_number_total             8707
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_collection       'Bruker XSCANS'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'XS (Sheldrick, 2008)'
_refine_diff_density_max         4.590
_refine_diff_density_min         -3.891
_refine_diff_density_rms         0.369
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.005
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     638
_refine_ls_number_reflns         8702
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0827
_refine_ls_R_factor_gt           0.0739
_refine_ls_restrained_S_all      1.005
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.1478P)²+508.7102P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2286
_refine_ls_wR_factor_ref         0.2389
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
 At 1.5 times of:
  All O(H,H) groups
2.a Rotating group:
 O2W(H2WA,H2WB), O3W(H3WA,H3WB), O4W(H4WA,H4WB), O1W(H1WA,H1WB)
2.b Aromatic/amide H refined with riding coordinates:
 C1(H1), C2(H2), C3(H3), C4(H4), C5(H5), C6(H6), C7(H7), C8(H8), C9(H9),
 C10(H10), C11(H11), C12(H12)
;
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.4515(6) 0.2516(4) 0.8252(8) 0.020(2) Uani 1 1 d . . . . .
H1 H 0.4850 0.2655 0.8908 0.024 Uiso 1 1 calc R . . . .
C2 C 0.6274(6) 0.2624(4) 0.5021(8) 0.021(2) Uani 1 1 d . . . . .
H2 H 0.6009 0.2831 0.4480 0.025 Uiso 1 1 calc R . . . .
C3 C 0.7935(6) 0.2085(4) 0.8868(8) 0.019(2) Uani 1 1 d . . . . .
H3 H 0.7587 0.1860 0.8573 0.023 Uiso 1 1 calc R . . . .
C4 C 0.4065(6) 0.2087(4) 0.6998(9) 0.019(2) Uani 1 1 d . . . . .
H4 H 0.4012 0.1864 0.6594 0.023 Uiso 1 1 calc R . . . .
C5 C 0.6258(5) 0.2621(4) 0.7532(8) 0.019(2) Uani 1 1 d . . . . .
H5 H 0.6536 0.2827 0.7545 0.022 Uiso 1 1 calc R . . . .
C6 C 0.5414(6) 0.2184(4) 0.7006(8) 0.019(2) Uani 1 1 d . . . . .
H6 H 0.4981 0.2014 0.6571 0.022 Uiso 1 1 calc R . . . .
C7 C 0.8743(6) 0.2515(4) 0.9223(8) 0.022(2) Uani 1 1 d . . . . .
H7 H 0.9070 0.2652 0.9217 0.026 Uiso 1 1 calc R . . . .
C8 C 0.6594(5) 0.2185(4) 0.6176(8) 0.018(2) Uani 1 1 d . . . . .
H8 H 0.6593 0.2018 0.6611 0.021 Uiso 1 1 calc R . . . .
C9 C 0.8001(7) 0.1528(4) 1.0677(11) 0.033(3) Uani 1 1 d . . . . .
H9 H 0.8478 0.1606 1.0987 0.040 Uiso 1 1 calc R . . . .
C10 C 0.7667(8) 0.1531(4) 0.4654(10) 0.034(3) Uani 1 1 d . . . . .
H10 H 0.7494 0.1607 0.4006 0.041 Uiso 1 1 calc R . . . .
C11 C 0.8078(9) 0.1163(5) 0.6014(12) 0.040(3) Uani 1 1 d . . . . .
H11 H 0.8239 0.0933 0.6476 0.048 Uiso 1 1 calc R . . . .
C12 C 0.7063(8) 0.1164(5) 1.0142(13) 0.043(4) Uani 1 1 d . . . . .
H12 H 0.6759 0.0934 0.9995 0.051 Uiso 1 1 calc R . . . .
N1 N 0.7141(5) 0.2175(3) 0.6232(7) 0.0171(18) Uani 1 1 d . . . . .
N2 N 0.5599(5) 0.2460(3) 0.6631(7) 0.0182(19) Uani 1 1 d . . . . .
N3 N 0.6031(5) 0.2460(3) 0.5434(7) 0.0163(18) Uani 1 1 d . . . . .
N4 N 0.5908(5) 0.2177(3) 0.8051(7) 0.0179(18) Uani 1 1 d . . . . .
N5 N 0.8308(5) 0.2158(3) 0.8614(7) 0.0185(19) Uani 1 1 d . . . . .
N6 N 0.4698(5) 0.2157(3) 0.8009(7) 0.0191(19) Uani 1 1 d . . . . .
N7 N 0.8515(5) 0.2636(3) 0.6614(6) 0.0151(17) Uani 1 1 d . . . . .
N8 N 0.8100(5) 0.2362(3) 0.9584(7) 0.0152(17) Uani 1 1 d . . . . .
N9 N 0.6917(5) 0.2464(3) 0.5453(7) 0.0185(19) Uani 1 1 d . . . . .
N10 N 0.6467(5) 0.2461(3) 0.8388(7) 0.0165(18) Uani 1 1 d . . . . .
N11 N 0.6367(5) 0.2358(3) 1.0169(7) 0.0171(18) Uani 1 1 d . . . . .
N12 N 0.7747(5) 0.1799(3) 0.5288(7) 0.021(2) Uani 1 1 d . . . . .
N13 N 0.8019(5) 0.1560(3) 0.6161(7) 0.021(2) Uani 1 1 d . . . . .
N14 N 0.8805(5) 0.2357(3) 0.7442(7) 0.0178(18) Uani 1 1 d . . . . .
N15 N 0.7809(7) 0.1127(4) 1.0680(12) 0.050(3) Uani 1 1 d . . . . .
N16 N 0.7868(8) 0.1128(4) 0.5067(11) 0.049(3) Uani 1 1 d . . . . .
N17 N 0.7460(5) 0.1794(3) 1.0203(7) 0.0207(19) Uani 1 1 d . . . . .
N18 N 0.6856(5) 0.1556(3) 0.9879(7) 0.021(2) Uani 1 1 d . . . . .
O1 O 0.5000 0.3167(3) 0.5000 0.031(3) Uani 1 2 d S T P . .
O2 O 0.7096(5) 0.3807(3) 0.6821(8) 0.041(2) Uani 1 1 d . . . . .
O3 O 0.6699(6) 0.4560(4) 0.5724(8) 0.062(4) Uani 1 1 d . . . . .
O4 O 0.6871(7) 0.4561(4) 0.7389(12) 0.070(4) Uani 1 1 d . . . . .
O5 O 0.4485(7) 0.4563(4) 0.6353(8) 0.070(4) Uani 1 1 d . . . . .
O6 O 0.3218(8) 0.5000 0.5540(12) 0.050(4) Uani 1 2 d S T P . .
O7 O 0.7324(8) 0.5000 0.9106(10) 0.051(4) Uani 1 2 d S T P . .
O8 O 0.5463(6) 0.0429(4) 0.3568(10) 0.066(4) Uani 1 1 d . . . . .
O9 O 0.4550(8) 0.0000 0.1622(11) 0.051(4) Uani 1 2 d S T P . .
O10 O 0.6683(8) 0.0436(4) 0.5671(9) 0.066(4) Uani 1 1 d . . . . .
O11 O 0.6900(8) 0.0433(4) 0.7360(9) 0.063(4) Uani 1 1 d . . . . .
O12 O 0.6702(5) 0.1188(3) 0.7962(7) 0.040(2) Uani 1 1 d . . . . .
O13 O 0.5989(5) 0.1049(3) 0.5838(7) 0.037(2) Uani 1 1 d . . . . .
O14 O 0.4852(5) 0.1046(3) 0.3865(7) 0.036(2) Uani 1 1 d . . . . .
O16 O 0.4432(8) 0.4718(5) 0.3993(11) 0.075(4) Uani 1 1 d . . . . .
O17 O 0.5435(8) 0.5280(5) 0.4866(12) 0.075(4) Uani 1 1 d . . . . .
O18 O 0.5000 0.1824(3) 0.5000 0.028(3) Uani 1 2 d S T P . .
O19 O 0.7923(7) 0.0000 0.7475(11) 0.051(4) Uani 1 2 d S T P . .
O20 O 0.5970(7) 0.4559(4) 0.7662(11) 0.061(4) Uani 1 1 d . . . . .
O21 O 0.5272(6) 0.3805(3) 0.7368(8) 0.042(2) Uani 1 1 d . . . . .
O22 O 0.4397(5) 0.3959(3) 0.5166(7) 0.039(2) Uani 1 1 d . . . . .
O23 O 0.4228(5) 0.3958(3) 0.3623(8) 0.038(2) Uani 1 1 d . . . . .
O24 O 0.4890(8) 0.0277(5) 0.4172(11) 0.071(4) Uani 1 1 d . . . . .
O25 O 0.4283(8) 0.0279(5) 0.4394(11) 0.072(4) Uani 1 1 d . . . . .
O26 O 0.6260(6) 0.1188(3) 0.4558(9) 0.042(2) Uani 1 1 d . . . . .
Co1 Co 0.7500 0.2500 0.5000 0.0135(4) Uani 1 2 d S T P . .
Co2 Co 0.81918(7) 0.18784(5) 0.74042(10) 0.0135(3) Uani 1 1 d . . . . .
Co3 Co 0.5000 0.25043(5) 0.5000 0.0068(4) Uani 1 2 d S T P . .
Co4 Co 0.7500 0.2500 1.0000 0.0137(4) Uani 1 2 d S T P . .
Co5 Co 0.57879(7) 0.18784(5) 0.89793(10) 0.0132(3) Uani 1 1 d . . . . .
Mo1 Mo 0.58872(6) 0.07833(3) 0.46853(8) 0.0218(3) Uani 1 1 d . . . . .
Mo2 Mo 0.62015(5) 0.07832(3) 0.70888(8) 0.0217(3) Uani 1 1 d . . . . .
Mo3 Mo 0.51787(6) 0.42107(3) 0.66544(8) 0.0230(3) Uani 1 1 d . . . . .
Mo4 Mo 0.64753(5) 0.42107(3) 0.62965(8) 0.0229(3) Uani 1 1 d . . . . .
Mo6 Mo 0.46819(10) 0.0000 0.26531(13) 0.0361(4) Uani 1 2 d S T P . .
Mo7 Mo 0.70292(9) 0.0000 0.67102(14) 0.0364(4) Uani 1 2 d S T P . .
Mo8 Mo 0.37614(11) 0.5000 0.53702(16) 0.0439(5) Uani 1 2 d S T P . .
Mo5 Mo 0.66101(11) 0.5000 0.78486(15) 0.0443(5) Uani 1 2 d S T P . .
P1 P 0.5000 0.5000 0.5000 0.0107(10) Uani 1 4 d S T P . .
P2 P 0.5000 0.0000 0.5000 0.0098(9) Uani 1 4 d S T P . .
V1 V 0.5000 0.36923(8) 0.5000 0.0200(6) Uani 1 2 d S T P . .
V2 V 0.5000 0.12980(8) 0.5000 0.0194(6) Uani 1 2 d S T P . .
O2W O 0.7672(5) 0.1322(3) 0.7407(8) 0.036(2) Uani 1 1 d . . . . .
H2WA H 0.7995 0.1188 0.7997 0.053 Uiso 1 1 d GR . . . .
H2WB H 0.7549 0.1137 0.6947 0.053 Uiso 1 1 d GR . . . .
O3W O 0.5266(5) 0.1326(3) 0.7939(7) 0.036(2) Uani 1 1 d . . . . .
H3WA H 0.4981 0.1199 0.7971 0.055 Uiso 1 1 d GR . . . .
H3WB H 0.5599 0.1136 0.8166 0.055 Uiso 1 1 d GR . . . .
O4W O 0.5601(6) 0.1519(4) 0.9813(8) 0.048(3) Uani 1 1 d . . . . .
H4WA H 0.5803 0.1563 1.0450 0.072 Uiso 1 1 d GR . . . .
H4WB H 0.5306 0.1298 0.9587 0.072 Uiso 1 1 d GR . . . .
O1W O 0.9219(6) 0.1521(4) 0.8621(8) 0.046(3) Uani 1 1 d . . . . .
H1WA H 0.9300 0.1317 0.9032 0.068 Uiso 1 1 d GR . . . .
H1WB H 0.9644 0.1548 0.8811 0.068 Uiso 1 1 d GR . . . .
O15 O 0.6009(5) 0.0435(4) 0.7687(10) 0.067(4) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
C1 N6 1.371(14) . ?
C1 N14 1.335(13) 8_455 ?
C2 N3 1.341(14) . ?
C2 N9 1.299(14) . ?
C3 N5 1.319(14) . ?
C3 N8 1.326(14) . ?
C4 N6 1.331(14) . ?
C4 N7 1.326(14) 8_455 ?
C5 N2 1.343(14) . ?
C5 N10 1.306(14) . ?
C6 N2 1.349(14) . ?
C6 N4 1.318(13) . ?
C7 N5 1.375(14) . ?
C7 N11 1.348(14) 7_657 ?
C8 N1 1.308(13) . ?
C8 N3 1.345(14) . ?
C9 N15 1.321(19) . ?
C9 N17 1.267(16) . ?
C10 N12 1.288(16) . ?
C10 N16 1.339(19) . ?
C11 N13 1.274(17) . ?
C11 N16 1.367(18) . ?
C12 N15 1.382(19) . ?
C12 N18 1.260(17) . ?
N1 N9 1.382(13) . ?
N1 Co2 2.091(9) . ?
N2 Co3 2.128(9) . ?
N3 Co3 2.125(8) . ?
N4 N10 1.377(12) . ?
N4 Co5 2.088(9) . ?
N5 Co2 2.135(9) . ?
N6 Co5 2.130(8) . ?
N7 C4 1.326(14) 8 ?
N7 N14 1.383(12) . ?
N7 Co1 2.140(8) . ?
N8 N11 1.376(13) 7_657 ?
N8 Co4 2.142(8) . ?
N9 Co1 2.118(9) . ?
N10 Co4 2.112(8) . ?
N11 C7 1.348(14) 7_657 ?
N11 N8 1.376(13) 7_657 ?
N11 Co5 2.097(9) . ?
N12 N13 1.384(13) . ?
N12 Co1 2.191(10) . ?
N13 Co2 2.161(9) . ?
N14 C1 1.335(14) 8 ?
N14 Co2 2.093(9) . ?
N17 N18 1.392(13) . ?
N17 Co4 2.203(10) . ?
N18 Co5 2.161(9) . ?
O1 Co3 2.028(11) . ?
O1 V1 1.606(11) . ?
O2 Mo4 1.665(8) . ?
O3 Mo4 1.818(10) . ?
O3 Mo8 1.939(10) 5_666 ?
O4 Mo4 1.784(10) . ?
O4 Mo5 1.914(10) . ?
O5 Mo3 1.782(10) . ?
O5 Mo8 1.913(10) . ?
O6 Mo8 1.595(14) . ?
O7 Mo5 1.597(13) . ?
O8 Mo1 1.808(10) . ?
O8 Mo6 1.927(10) . ?
O9 Mo6 1.617(13) . ?
O10 Mo1 1.802(10) . ?
O10 Mo7 1.920(10) . ?
O11 Mo2 1.808(10) . ?
O11 Mo7 1.931(10) . ?
O12 Mo2 1.663(8) . ?
O13 Mo1 2.047(9) . ?
O13 Mo2 2.055(9) . ?
O13 V2 1.937(9) . ?
O14 Mo1 2.047(9) . ?
O14 Mo2 2.048(9) 2_656 ?
O14 V2 1.936(9) . ?
O16 O16 1.72(3) 6_565 ?
O16 O17 1.81(2) 5_666 ?
O16 O17 1.80(2) 6_565 ?
O16 Mo3 2.508(15) 2_656 ?
O16 Mo4 2.495(14) 2_656 ?
O16 Mo5 2.492(15) 5_666 ?
O16 P1 1.542(13) . ?
O17 O16 1.80(2) 6_565 ?
O17 O16 1.81(2) 5_666 ?
O17 O17 1.71(3) 6_565 ?
O17 Mo3 2.496(15) 5_666 ?
O17 Mo4 2.519(15) 6_565 ?
O17 Mo8 2.489(15) 5_666 ?
O17 P1 1.534(13) . ?
O18 Co3 2.081(11) . ?
O18 V2 1.609(11) . ?
O19 Mo7 1.606(13) . ?
O20 Mo3 1.808(10) . ?
O20 Mo5 1.941(10) . ?
O21 Mo3 1.671(8) . ?
O22 Mo3 2.029(9) . ?
O22 Mo4 2.028(9) 2_656 ?
O22 V1 1.918(9) . ?
O23 Mo3 2.026(9) 2_656 ?
O23 Mo4 2.027(9) 2_656 ?
O23 V1 1.927(9) . ?
O24 O24 1.69(3) 6 ?
O24 Mo1 2.507(14) . ?
O24 Mo2 2.504(14) 2_656 ?
O24 Mo6 2.508(14) . ?
O24 P2 1.546(13) . ?
O25 O25 1.71(3) 6 ?
O25 Mo1 2.498(14) 2_656 ?
O25 Mo2 2.506(14) 2_656 ?
O25 Mo7 2.514(15) 5_656 ?
O25 P2 1.547(13) . ?
O26 Mo1 1.661(8) . ?
Co1 N7 2.140(8) 7_656 ?
Co1 N9 2.119(9) 7_656 ?
Co1 N12 2.191(10) 7_656 ?
Co2 O2W 2.148(9) . ?
Co2 O1W 2.158(10) . ?
Co3 N2 2.128(9) 2_656 ?
Co3 N3 2.125(8) 2_656 ?
Co4 N8 2.142(8) 7_657 ?
Co4 N10 2.112(8) 7_657 ?
Co4 N17 2.203(10) 7_657 ?
Co5 O3W 2.137(9) . ?
Co5 O4W 2.150(10) . ?
Mo1 O25 2.498(14) 2_656 ?
Mo1 V2 3.0885(17) . ?
Mo2 O14 2.048(9) 2_656 ?
Mo2 O24 2.504(14) 2_656 ?
Mo2 O25 2.506(14) 2_656 ?
Mo2 V2 3.0912(17) . ?
Mo2 O15 1.796(10) . ?
Mo3 O16 2.508(15) 2_656 ?
Mo3 O17 2.496(15) 5_666 ?
Mo3 O23 2.026(9) 2_656 ?
Mo3 V1 3.0840(18) . ?
Mo4 O16 2.494(14) 2_656 ?
Mo4 O17 2.519(15) 6_565 ?
Mo4 O22 2.028(9) 2_656 ?
Mo4 O23 2.027(9) 2_656 ?
Mo4 V1 3.0841(18) . ?
Mo6 O8 1.927(10) 6 ?
Mo6 O24 2.508(14) 6 ?
Mo6 O15 1.917(10) 5_656 ?
Mo6 O15 1.917(10) 2_656 ?
Mo7 O10 1.920(10) 6 ?
Mo7 O11 1.931(10) 6 ?
Mo7 O25 2.514(15) 5_656 ?
Mo7 O25 2.514(15) 2_656 ?
Mo8 O3 1.938(10) 2_656 ?
Mo8 O3 1.938(10) 5_666 ?
Mo8 O5 1.913(10) 6_565 ?
Mo8 O17 2.489(15) 2_656 ?
Mo8 O17 2.489(15) 5_666 ?
Mo5 O4 1.914(10) 6_565 ?
Mo5 O16 2.492(15) 5_666 ?
Mo5 O16 2.492(15) 2_656 ?
Mo5 O20 1.941(10) 6_565 ?
P1 O16 1.542(13) 2_656 ?
P1 O16 1.542(13) 5_666 ?
P1 O16 1.542(13) 6_565 ?
P1 O17 1.534(13) 5_666 ?
P1 O17 1.534(13) 2_656 ?
P1 O17 1.534(13) 6_565 ?
P2 O24 1.546(13) 2_656 ?
P2 O24 1.546(13) 5_656 ?
P2 O24 1.546(13) 6 ?
P2 O25 1.547(14) 2_656 ?
P2 O25 1.547(13) 5_656 ?
P2 O25 1.547(13) 6 ?
V1 O22 1.918(9) 2_656 ?
V1 O23 1.927(9) 2_656 ?
V1 Mo3 3.0840(18) 2_656 ?
V1 Mo4 3.0841(18) 2_656 ?
V2 O13 1.937(9) 2_656 ?
V2 O14 1.936(9) 2_656 ?
V2 Mo1 3.0885(17) 2_656 ?
V2 Mo2 3.0912(17) 2_656 ?
O15 Mo6 1.917(10) 5_656 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N14 C1 N6 112.6(9) 8_455 . ?
N9 C2 N3 113.0(10) . . ?
N5 C3 N8 113.8(10) . . ?
N7 C4 N6 114.2(10) 8_455 . ?
N10 C5 N2 113.3(10) . . ?
N4 C6 N2 113.4(9) . . ?
N11 C7 N5 111.3(9) 7_657 . ?
N1 C8 N3 114.2(9) . . ?
N17 C9 N15 112.1(12) . . ?
N12 C10 N16 110.0(11) . . ?
N13 C11 N16 109.2(12) . . ?
N18 C12 N15 109.8(13) . . ?
C8 N1 N9 104.2(8) . . ?
C8 N1 Co2 127.4(7) . . ?
N9 N1 Co2 127.6(6) . . ?
C5 N2 C6 101.8(9) . . ?
C5 N2 Co3 133.8(8) . . ?
C6 N2 Co3 123.7(7) . . ?
C2 N3 C8 101.7(9) . . ?
C2 N3 Co3 133.5(7) . . ?
C8 N3 Co3 124.3(7) . . ?
C6 N4 N10 105.0(8) . . ?
C6 N4 Co5 127.1(7) . . ?
N10 N4 Co5 127.2(6) . . ?
C3 N5 C7 103.1(9) . . ?
C3 N5 Co2 130.9(7) . . ?
C7 N5 Co2 125.5(7) . . ?
C1 N6 Co5 126.2(7) . . ?
C4 N6 C1 101.9(9) . . ?
C4 N6 Co5 131.1(7) . . ?
C4 N7 N14 105.8(8) 8 . ?
C4 N7 Co1 129.5(7) 8 . ?
N14 N7 Co1 122.7(7) . . ?
C3 N8 N11 106.3(8) . 7_657 ?
C3 N8 Co4 129.6(7) . . ?
N11 N8 Co4 122.1(6) 7_657 . ?
C2 N9 N1 106.9(9) . . ?
C2 N9 Co1 131.4(8) . . ?
N1 N9 Co1 120.9(6) . . ?
C5 N10 N4 106.4(8) . . ?
C5 N10 Co4 131.1(7) . . ?
N4 N10 Co4 121.6(6) . . ?
C7 N11 N8 105.6(8) 7_657 7_657 ?
C7 N11 Co5 128.4(7) 7_657 . ?
N8 N11 Co5 125.7(6) 7_657 . ?
C10 N12 N13 107.1(10) . . ?
C10 N12 Co1 125.1(9) . . ?
N13 N12 Co1 127.8(7) . . ?
C11 N13 N12 108.0(10) . . ?
C11 N13 Co2 132.3(9) . . ?
N12 N13 Co2 119.5(7) . . ?
C1 N14 N7 105.4(8) 8 . ?
C1 N14 Co2 129.3(7) 8 . ?
N7 N14 Co2 125.1(6) . . ?
C9 N15 C12 104.0(11) . . ?
C10 N16 C11 105.7(11) . . ?
C9 N17 N18 106.6(10) . . ?
C9 N17 Co4 126.0(9) . . ?
N18 N17 Co4 127.4(7) . . ?
C12 N18 N17 107.4(10) . . ?
C12 N18 Co5 132.9(9) . . ?
N17 N18 Co5 119.4(7) . . ?
V1 O1 Co3 180.0 . . ?
Mo4 O3 Mo8 140.3(8) . 5_666 ?
Mo4 O4 Mo5 142.3(8) . . ?
Mo3 O5 Mo8 142.7(8) . . ?
Mo1 O8 Mo6 142.6(8) . . ?
Mo1 O10 Mo7 141.5(8) . . ?
Mo2 O11 Mo7 142.2(8) . . ?
Mo1 O13 Mo2 132.9(5) . . ?
V2 O13 Mo1 101.6(4) . . ?
V2 O13 Mo2 101.5(4) . . ?
Mo1 O14 Mo2 133.3(5) . 2_656 ?
V2 O14 Mo1 101.7(4) . . ?
V2 O14 Mo2 101.8(4) . 2_656 ?
O16 O16 O17 89.8(7) 6_565 6_565 ?
O16 O16 O17 89.8(7) 6_565 5_666 ?
O16 O16 Mo3 128.3(3) 6_565 2_656 ?
O16 O16 Mo4 128.5(3) 6_565 2_656 ?
O16 O16 Mo5 69.8(3) 6_565 5_666 ?
O17 O16 O17 89.8(9) 6_565 5_666 ?
O17 O16 Mo3 134.0(9) 5_666 2_656 ?
O17 O16 Mo3 68.6(7) 6_565 2_656 ?
O17 O16 Mo4 69.6(7) 5_666 2_656 ?
O17 O16 Mo4 134.4(9) 6_565 2_656 ?
O17 O16 Mo5 131.6(9) 6_565 5_666 ?
O17 O16 Mo5 131.5(9) 5_666 5_666 ?
Mo4 O16 Mo3 96.7(5) 2_656 2_656 ?
Mo5 O16 Mo3 90.0(5) 5_666 2_656 ?
Mo5 O16 Mo4 89.1(4) 5_666 2_656 ?
P1 O16 O16 56.0(6) . 6_565 ?
P1 O16 O17 54.0(6) . 6_565 ?
P1 O16 O17 53.8(6) . 5_666 ?
P1 O16 Mo3 122.5(8) . 2_656 ?
P1 O16 Mo4 123.3(8) . 2_656 ?
P1 O16 Mo5 125.8(8) . 5_666 ?
O16 O17 O16 90.2(9) 6_565 5_666 ?
O16 O17 Mo3 134.1(9) 5_666 5_666 ?
O16 O17 Mo3 69.3(7) 6_565 5_666 ?
O16 O17 Mo4 68.1(6) 5_666 6_565 ?
O16 O17 Mo4 133.8(9) 6_565 6_565 ?
O16 O17 Mo8 131.4(9) 5_666 5_666 ?
O16 O17 Mo8 131.7(9) 6_565 5_666 ?
O17 O17 O16 90.2(7) 6_565 6_565 ?
O17 O17 O16 90.2(7) 6_565 5_666 ?
O17 O17 Mo3 128.7(3) 6_565 5_666 ?
O17 O17 Mo4 128.2(3) 6_565 6_565 ?
O17 O17 Mo8 69.9(3) 6_565 5_666 ?
Mo3 O17 Mo4 96.5(5) 5_666 6_565 ?
Mo8 O17 Mo3 89.2(5) 5_666 5_666 ?
Mo8 O17 Mo4 89.7(5) 5_666 6_565 ?
P1 O17 O16 54.2(6) . 5_666 ?
P1 O17 O16 54.4(6) . 6_565 ?
P1 O17 O17 56.1(6) . 6_565 ?
P1 O17 Mo3 123.7(8) . 5_666 ?
P1 O17 Mo4 122.3(8) . 6_565 ?
P1 O17 Mo8 126.0(8) . 5_666 ?
V2 O18 Co3 180.0 . . ?
Mo3 O20 Mo5 141.1(8) . . ?
Mo4 O22 Mo3 134.6(5) 2_656 . ?
V1 O22 Mo3 102.7(4) . . ?
V1 O22 Mo4 102.8(4) . 2_656 ?
Mo4 O23 Mo3 134.5(5) 2_656 2_656 ?
V1 O23 Mo3 102.5(4) . 2_656 ?
V1 O23 Mo4 102.5(4) . 2_656 ?
O24 O24 Mo1 128.2(3) 6 . ?
O24 O24 Mo2 128.2(3) 6 2_656 ?
O24 O24 Mo6 70.3(3) 6 . ?
Mo1 O24 Mo6 89.7(4) . . ?
Mo2 O24 Mo1 97.2(5) 2_656 . ?
Mo2 O24 Mo6 89.0(4) 2_656 . ?
P2 O24 O24 56.8(5) . 6 ?
P2 O24 Mo1 122.2(8) . . ?
P2 O24 Mo2 122.5(7) . 2_656 ?
P2 O24 Mo6 127.0(8) . . ?
O25 O25 Mo1 128.1(3) 6 2_656 ?
O25 O25 Mo2 128.0(3) 6 2_656 ?
O25 O25 Mo7 70.2(3) 6 5_656 ?
Mo1 O25 Mo2 97.4(5) 2_656 2_656 ?
Mo1 O25 Mo7 89.0(4) 2_656 5_656 ?
Mo2 O25 Mo7 89.6(4) 2_656 5_656 ?
P2 O25 O25 56.5(6) . 6 ?
P2 O25 Mo1 122.6(7) . 2_656 ?
P2 O25 Mo2 122.3(7) . 2_656 ?
P2 O25 Mo7 126.7(8) . 5_656 ?
N7 Co1 N7 180.0 7_656 . ?
N7 Co1 N12 89.7(3) . 7_656 ?
N7 Co1 N12 90.3(3) . . ?
N7 Co1 N12 90.3(3) 7_656 7_656 ?
N7 Co1 N12 89.7(3) 7_656 . ?
N9 Co1 N7 89.4(3) . . ?
N9 Co1 N7 90.6(3) . 7_656 ?
N9 Co1 N7 90.6(3) 7_656 . ?
N9 Co1 N7 89.4(3) 7_656 7_656 ?
N9 Co1 N9 180.00(18) 7_656 . ?
N9 Co1 N12 91.0(3) . . ?
N9 Co1 N12 91.0(3) 7_656 7_656 ?
N9 Co1 N12 89.0(3) . 7_656 ?
N9 Co1 N12 89.0(3) 7_656 . ?
N12 Co1 N12 180.00(10) 7_656 . ?
N1 Co2 N5 90.5(3) . . ?
N1 Co2 N13 88.7(3) . . ?
N1 Co2 N14 96.4(4) . . ?
N1 Co2 O2W 90.2(4) . . ?
N1 Co2 O1W 174.2(4) . . ?
N5 Co2 N13 175.7(4) . . ?
N5 Co2 O2W 88.1(4) . . ?
N5 Co2 O1W 88.7(4) . . ?
N14 Co2 N5 96.6(4) . . ?
N14 Co2 N13 87.7(4) . . ?
N14 Co2 O2W 171.8(4) . . ?
N14 Co2 O1W 89.4(4) . . ?
O2W Co2 N13 87.8(4) . . ?
O2W Co2 O1W 84.0(4) . . ?
O1W Co2 N13 91.8(4) . . ?
N2 Co3 N2 172.8(5) . 2_656 ?
N3 Co3 N2 89.9(3) . 2_656 ?
N3 Co3 N2 89.6(3) . . ?
N3 Co3 N2 89.9(3) 2_656 . ?
N3 Co3 N2 89.6(3) 2_656 2_656 ?
N3 Co3 N3 172.6(5) . 2_656 ?
O1 Co3 N2 93.6(3) . 2_656 ?
O1 Co3 N2 93.6(3) . . ?
O1 Co3 N3 93.7(2) . 2_656 ?
O1 Co3 N3 93.7(2) . . ?
O1 Co3 O18 180.0 . . ?
O18 Co3 N2 86.4(3) . 2_656 ?
O18 Co3 N2 86.4(3) . . ?
O18 Co3 N3 86.3(2) . . ?
O18 Co3 N3 86.3(2) . 2_656 ?
N8 Co4 N8 180.0 7_657 . ?
N8 Co4 N17 89.3(3) 7_657 7_657 ?
N8 Co4 N17 90.7(3) 7_657 . ?
N8 Co4 N17 90.7(3) . 7_657 ?
N8 Co4 N17 89.3(3) . . ?
N10 Co4 N8 89.4(3) . 7_657 ?
N10 Co4 N8 89.4(3) 7_657 . ?
N10 Co4 N8 90.6(3) . . ?
N10 Co4 N8 90.6(3) 7_657 7_657 ?
N10 Co4 N10 180.0(5) . 7_657 ?
N10 Co4 N17 90.7(3) . . ?
N10 Co4 N17 90.7(3) 7_657 7_657 ?
N10 Co4 N17 89.3(3) 7_657 . ?
N10 Co4 N17 89.3(3) . 7_657 ?
N17 Co4 N17 180.00(10) 7_657 . ?
N4 Co5 N6 90.4(4) . . ?
N4 Co5 N11 96.1(4) . . ?
N4 Co5 N18 89.2(4) . . ?
N4 Co5 O3W 90.2(4) . . ?
N4 Co5 O4W 174.1(4) . . ?
N6 Co5 N18 175.7(4) . . ?
N6 Co5 O3W 87.9(4) . . ?
N6 Co5 O4W 88.8(4) . . ?
N11 Co5 N6 96.7(4) . . ?
N11 Co5 N18 87.6(4) . . ?
N11 Co5 O3W 172.1(4) . . ?
N11 Co5 O4W 89.8(4) . . ?
O3W Co5 N18 87.9(4) . . ?
O3W Co5 O4W 83.9(4) . . ?
O4W Co5 N18 91.1(4) . . ?
O8 Mo1 O13 154.0(5) . . ?
O8 Mo1 O14 89.2(4) . . ?
O8 Mo1 O24 64.4(5) . . ?
O8 Mo1 O25 96.3(6) . 2_656 ?
O8 Mo1 V2 124.4(3) . . ?
O10 Mo1 O8 95.9(6) . . ?
O10 Mo1 O13 89.6(4) . . ?
O10 Mo1 O14 154.7(5) . . ?
O10 Mo1 O24 97.4(6) . . ?
O10 Mo1 O25 65.5(5) . 2_656 ?
O10 Mo1 V2 124.9(3) . . ?
O13 Mo1 O24 89.8(4) . . ?
O13 Mo1 O25 63.0(4) . 2_656 ?
O13 Mo1 V2 37.9(2) . . ?
O14 Mo1 O13 75.7(4) . . ?
O14 Mo1 O24 62.7(4) . . ?
O14 Mo1 O25 89.4(4) . 2_656 ?
O14 Mo1 V2 37.9(2) . . ?
O24 Mo1 V2 73.5(3) . . ?
O25 Mo1 O24 42.8(4) 2_656 . ?
O25 Mo1 V2 73.5(3) 2_656 . ?
O26 Mo1 O8 104.4(6) . . ?
O26 Mo1 O10 103.0(6) . . ?
O26 Mo1 O13 99.0(5) . . ?
O26 Mo1 O14 99.6(5) . . ?
O26 Mo1 O24 157.8(5) . . ?
O26 Mo1 O25 157.5(5) . 2_656 ?
O26 Mo1 V2 101.2(4) . . ?
O11 Mo2 O13 89.1(4) . . ?
O11 Mo2 O14 153.9(5) . 2_656 ?
O11 Mo2 O24 96.7(6) . 2_656 ?
O11 Mo2 O25 64.8(5) . 2_656 ?
O11 Mo2 V2 124.3(3) . . ?
O12 Mo2 O11 103.9(6) . . ?
O12 Mo2 O13 99.4(5) . . ?
O12 Mo2 O14 99.4(5) . 2_656 ?
O12 Mo2 O24 157.6(5) . 2_656 ?
O12 Mo2 O25 157.7(5) . 2_656 ?
O12 Mo2 V2 101.3(3) . . ?
O12 Mo2 O15 103.3(6) . . ?
O13 Mo2 O24 89.6(4) . 2_656 ?
O13 Mo2 O25 62.8(4) . 2_656 ?
O13 Mo2 V2 37.9(2) . . ?
O14 Mo2 O13 75.7(3) 2_656 . ?
O14 Mo2 O24 62.8(4) 2_656 2_656 ?
O14 Mo2 O25 89.2(4) 2_656 2_656 ?
O14 Mo2 V2 37.8(2) 2_656 . ?
O24 Mo2 O25 42.8(4) 2_656 2_656 ?
O24 Mo2 V2 73.5(3) 2_656 . ?
O25 Mo2 V2 73.3(3) 2_656 . ?
O15 Mo2 O11 96.2(6) . . ?
O15 Mo2 O13 154.7(5) . . ?
O15 Mo2 O14 89.5(4) . 2_656 ?
O15 Mo2 O24 65.2(5) . 2_656 ?
O15 Mo2 O25 97.1(6) . 2_656 ?
O15 Mo2 V2 124.8(3) . . ?
O5 Mo3 O16 96.0(6) . 2_656 ?
O5 Mo3 O17 64.6(5) . 5_666 ?
O5 Mo3 O20 95.7(6) . . ?
O5 Mo3 O22 89.9(4) . . ?
O5 Mo3 O23 153.0(5) . 2_656 ?
O5 Mo3 V1 125.0(3) . . ?
O16 Mo3 V1 73.8(4) 2_656 . ?
O17 Mo3 O16 42.2(4) 5_666 2_656 ?
O17 Mo3 V1 74.1(3) 5_666 . ?
O20 Mo3 O16 65.0(5) . 2_656 ?
O20 Mo3 O17 96.4(6) . 5_666 ?
O20 Mo3 O22 153.0(5) . . ?
O20 Mo3 O23 89.0(4) . 2_656 ?
O20 Mo3 V1 124.5(3) . . ?
O21 Mo3 O5 105.1(6) . . ?
O21 Mo3 O16 156.8(5) . 2_656 ?
O21 Mo3 O17 159.3(5) . 5_666 ?
O21 Mo3 O20 102.7(6) . . ?
O21 Mo3 O22 101.3(5) . . ?
O21 Mo3 O23 99.8(5) . 2_656 ?
O21 Mo3 V1 101.0(3) . . ?
O22 Mo3 O16 88.2(5) . 2_656 ?
O22 Mo3 O17 62.3(4) . 5_666 ?
O22 Mo3 V1 37.4(3) . . ?
O23 Mo3 O16 62.0(4) 2_656 2_656 ?
O23 Mo3 O17 88.4(5) 2_656 5_666 ?
O23 Mo3 O22 74.8(4) 2_656 . ?
O23 Mo3 V1 37.6(3) 2_656 . ?
O2 Mo4 O3 102.2(6) . . ?
O2 Mo4 O4 104.7(6) . . ?
O2 Mo4 O16 159.4(5) . 2_656 ?
O2 Mo4 O17 156.7(5) . 6_565 ?
O2 Mo4 O22 100.0(5) . 2_656 ?
O2 Mo4 O23 101.4(5) . 2_656 ?
O2 Mo4 V1 101.2(3) . . ?
O3 Mo4 O16 96.8(6) . 2_656 ?
O3 Mo4 O17 65.3(5) . 6_565 ?
O3 Mo4 O22 89.3(4) . 2_656 ?
O3 Mo4 O23 153.5(5) . 2_656 ?
O3 Mo4 V1 124.6(3) . . ?
O4 Mo4 O3 95.8(6) . . ?
O4 Mo4 O16 64.9(5) . 2_656 ?
O4 Mo4 O17 96.4(6) . 6_565 ?
O4 Mo4 O22 153.0(5) . 2_656 ?
O4 Mo4 O23 89.8(4) . 2_656 ?
O4 Mo4 V1 125.1(3) . . ?
O16 Mo4 O17 42.3(4) 2_656 6_565 ?
O16 Mo4 V1 74.0(4) 2_656 . ?
O17 Mo4 V1 73.8(4) 6_565 . ?
O22 Mo4 O16 88.2(5) 2_656 2_656 ?
O22 Mo4 O17 61.9(5) 2_656 6_565 ?
O22 Mo4 V1 37.3(3) 2_656 . ?
O23 Mo4 O16 62.3(5) 2_656 2_656 ?
O23 Mo4 O17 88.4(5) 2_656 6_565 ?
O23 Mo4 O22 74.8(4) 2_656 2_656 ?
O23 Mo4 V1 37.6(3) 2_656 . ?
O8 Mo6 O8 85.8(8) 6 . ?
O8 Mo6 O24 90.4(6) . 6 ?
O8 Mo6 O24 90.4(6) 6 . ?
O8 Mo6 O24 63.1(5) 6 6 ?
O8 Mo6 O24 63.1(5) . . ?
O9 Mo6 O8 103.2(6) . . ?
O9 Mo6 O8 103.2(6) . 6 ?
O9 Mo6 O24 160.2(3) . 6 ?
O9 Mo6 O24 160.2(3) . . ?
O9 Mo6 O15 103.2(6) . 5_656 ?
O9 Mo6 O15 103.2(6) . 2_656 ?
O24 Mo6 O24 39.5(6) 6 . ?
O15 Mo6 O8 153.6(6) 5_656 . ?
O15 Mo6 O8 153.6(6) 2_656 6 ?
O15 Mo6 O8 87.1(4) 2_656 . ?
O15 Mo6 O8 87.1(4) 5_656 6 ?
O15 Mo6 O24 63.8(5) 2_656 . ?
O15 Mo6 O24 91.6(6) 5_656 . ?
O15 Mo6 O24 91.6(6) 2_656 6 ?
O15 Mo6 O24 63.8(5) 5_656 6 ?
O15 Mo6 O15 88.0(8) 5_656 2_656 ?
O10 Mo7 O10 88.1(8) . 6 ?
O10 Mo7 O11 154.2(6) . 6 ?
O10 Mo7 O11 86.9(4) 6 6 ?
O10 Mo7 O11 154.2(6) 6 . ?
O10 Mo7 O11 86.9(4) . . ?
O10 Mo7 O25 63.9(5) 6 5_656 ?
O10 Mo7 O25 91.8(6) . 5_656 ?
O10 Mo7 O25 63.9(5) . 2_656 ?
O10 Mo7 O25 91.8(6) 6 2_656 ?
O11 Mo7 O11 86.6(8) 6 . ?
O11 Mo7 O25 63.3(5) . 2_656 ?
O11 Mo7 O25 90.9(6) 6 2_656 ?
O11 Mo7 O25 63.3(5) 6 5_656 ?
O11 Mo7 O25 90.9(6) . 5_656 ?
O19 Mo7 O10 103.1(6) . . ?
O19 Mo7 O10 103.1(6) . 6 ?
O19 Mo7 O11 102.7(6) . 6 ?
O19 Mo7 O11 102.7(6) . . ?
O19 Mo7 O25 160.1(3) . 5_656 ?
O19 Mo7 O25 160.1(3) . 2_656 ?
O25 Mo7 O25 39.7(6) 5_656 2_656 ?
O3 Mo8 O3 88.0(7) 2_656 5_666 ?
O3 Mo8 O17 92.8(6) 5_666 5_666 ?
O3 Mo8 O17 64.6(5) 5_666 2_656 ?
O3 Mo8 O17 64.6(5) 2_656 5_666 ?
O3 Mo8 O17 92.8(6) 2_656 2_656 ?
O5 Mo8 O3 86.6(4) . 2_656 ?
O5 Mo8 O3 86.6(4) 6_565 5_666 ?
O5 Mo8 O3 155.6(7) . 5_666 ?
O5 Mo8 O3 155.6(7) 6_565 2_656 ?
O5 Mo8 O5 88.6(8) 6_565 . ?
O5 Mo8 O17 91.9(6) . 2_656 ?
O5 Mo8 O17 63.4(5) 6_565 2_656 ?
O5 Mo8 O17 91.9(6) 6_565 5_666 ?
O5 Mo8 O17 63.4(5) . 5_666 ?
O6 Mo8 O3 101.9(6) . 2_656 ?
O6 Mo8 O3 101.9(6) . 5_666 ?
O6 Mo8 O5 102.5(6) . 6_565 ?
O6 Mo8 O5 102.5(6) . . ?
O6 Mo8 O17 159.9(3) . 2_656 ?
O6 Mo8 O17 159.9(3) . 5_666 ?
O17 Mo8 O17 40.2(6) 2_656 5_666 ?
O4 Mo5 O4 89.1(8) 6_565 . ?
O4 Mo5 O16 63.6(5) 6_565 5_666 ?
O4 Mo5 O16 92.3(6) . 5_666 ?
O4 Mo5 O16 63.6(5) . 2_656 ?
O4 Mo5 O16 92.3(6) 6_565 2_656 ?
O4 Mo5 O20 86.2(4) . . ?
O4 Mo5 O20 155.3(6) . 6_565 ?
O4 Mo5 O20 155.3(6) 6_565 . ?
O4 Mo5 O20 86.2(4) 6_565 6_565 ?
O7 Mo5 O4 102.3(6) . . ?
O7 Mo5 O4 102.3(6) . 6_565 ?
O7 Mo5 O16 159.8(3) . 2_656 ?
O7 Mo5 O16 159.8(3) . 5_666 ?
O7 Mo5 O20 102.4(6) . . ?
O7 Mo5 O20 102.4(6) . 6_565 ?
O16 Mo5 O16 40.5(6) 2_656 5_666 ?
O20 Mo5 O16 63.9(5) 6_565 5_666 ?
O20 Mo5 O16 92.3(6) . 5_666 ?
O20 Mo5 O16 92.3(6) 6_565 2_656 ?
O20 Mo5 O16 63.9(5) . 2_656 ?
O20 Mo5 O20 88.0(7) . 6_565 ?
O16 P1 O16 112.0(11) 5_666 6_565 ?
O16 P1 O16 68.0(11) . 6_565 ?
O16 P1 O16 180.0(9) 6_565 2_656 ?
O16 P1 O16 112.0(11) . 2_656 ?
O16 P1 O16 68.0(11) 5_666 2_656 ?
O16 P1 O16 180.0(15) . 5_666 ?
O17 P1 O16 71.6(8) 6_565 . ?
O17 P1 O16 72.1(8) . 5_666 ?
O17 P1 O16 71.6(8) 2_656 5_666 ?
O17 P1 O16 72.1(8) 2_656 6_565 ?
O17 P1 O16 71.6(8) 5_666 2_656 ?
O17 P1 O16 72.1(8) 5_666 . ?
O17 P1 O16 107.9(8) 5_666 5_666 ?
O17 P1 O16 72.1(8) 6_565 2_656 ?
O17 P1 O16 108.4(8) 2_656 . ?
O17 P1 O16 108.4(8) 5_666 6_565 ?
O17 P1 O16 108.4(8) . 2_656 ?
O17 P1 O16 107.9(8) 2_656 2_656 ?
O17 P1 O16 107.9(8) 6_565 6_565 ?
O17 P1 O16 107.9(8) . . ?
O17 P1 O16 71.6(8) . 6_565 ?
O17 P1 O16 108.4(8) 6_565 5_666 ?
O17 P1 O17 180.0(12) 6_565 2_656 ?
O17 P1 O17 180.0 . 5_666 ?
O17 P1 O17 67.8(11) . 6_565 ?
O17 P1 O17 112.2(11) 5_666 6_565 ?
O17 P1 O17 67.8(11) 5_666 2_656 ?
O17 P1 O17 112.2(11) . 2_656 ?
O24 P2 O24 113.5(11) 6 5_656 ?
O24 P2 O24 66.5(11) 6 . ?
O24 P2 O24 180.0 6 2_656 ?
O24 P2 O24 180.0(13) 5_656 . ?
O24 P2 O24 113.5(11) 2_656 . ?
O24 P2 O24 66.5(11) 2_656 5_656 ?
O24 P2 O25 107.6(7) 2_656 6 ?
O24 P2 O25 72.4(7) 6 6 ?
O24 P2 O25 72.4(7) 5_656 5_656 ?
O24 P2 O25 107.6(7) 2_656 5_656 ?
O24 P2 O25 72.4(7) 2_656 . ?
O24 P2 O25 72.4(7) . 2_656 ?
O24 P2 O25 72.4(7) . . ?
O24 P2 O25 107.6(7) 6 2_656 ?
O24 P2 O25 107.6(7) 5_656 . ?
O24 P2 O25 107.6(7) 6 . ?
O24 P2 O25 107.6(7) . 5_656 ?
O24 P2 O25 72.4(7) 5_656 6 ?
O24 P2 O25 107.6(7) . 6 ?
O24 P2 O25 72.4(7) 2_656 2_656 ?
O24 P2 O25 107.6(7) 5_656 2_656 ?
O24 P2 O25 72.4(7) 6 5_656 ?
O25 P2 O25 67.0(11) 2_656 5_656 ?
O25 P2 O25 180.0(13) 6 2_656 ?
O25 P2 O25 67.0(11) 6 . ?
O25 P2 O25 113.0(11) 2_656 . ?
O25 P2 O25 113.0(11) 6 5_656 ?
O25 P2 O25 180.0(11) 5_656 . ?
O1 V1 O22 115.1(3) . . ?
O1 V1 O22 115.1(3) . 2_656 ?
O1 V1 O23 115.0(3) . . ?
O1 V1 O23 115.0(3) . 2_656 ?
O1 V1 Mo3 120.95(5) . 2_656 ?
O1 V1 Mo3 120.95(4) . . ?
O1 V1 Mo4 120.95(5) . 2_656 ?
O1 V1 Mo4 120.95(5) . . ?
O22 V1 O22 129.7(7) 2_656 . ?
O22 V1 O23 79.7(4) . . ?
O22 V1 O23 79.7(4) 2_656 . ?
O22 V1 O23 79.7(4) . 2_656 ?
O22 V1 O23 79.7(4) 2_656 2_656 ?
O22 V1 Mo3 109.3(3) 2_656 . ?
O22 V1 Mo3 109.3(3) . 2_656 ?
O22 V1 Mo3 39.9(3) . . ?
O22 V1 Mo3 39.9(3) 2_656 2_656 ?
O22 V1 Mo4 39.9(3) . 2_656 ?
O22 V1 Mo4 109.3(3) . . ?
O22 V1 Mo4 39.9(3) 2_656 . ?
O22 V1 Mo4 109.3(3) 2_656 2_656 ?
O23 V1 O23 130.1(7) . 2_656 ?
O23 V1 Mo3 109.5(3) 2_656 2_656 ?
O23 V1 Mo3 39.9(3) . 2_656 ?
O23 V1 Mo3 109.5(3) . . ?
O23 V1 Mo3 39.9(3) 2_656 . ?
O23 V1 Mo4 109.5(3) 2_656 2_656 ?
O23 V1 Mo4 39.9(3) 2_656 . ?
O23 V1 Mo4 39.9(3) . 2_656 ?
O23 V1 Mo4 109.5(3) . . ?
Mo3 V1 Mo3 118.10(9) . 2_656 ?
Mo3 V1 Mo4 74.72(5) 2_656 . ?
Mo3 V1 Mo4 74.60(5) . . ?
Mo4 V1 Mo3 74.61(5) 2_656 2_656 ?
Mo4 V1 Mo3 74.72(5) 2_656 . ?
Mo4 V1 Mo4 118.09(9) 2_656 . ?
O13 V2 O13 133.7(7) . 2_656 ?
O13 V2 Mo1 40.5(3) . . ?
O13 V2 Mo1 40.5(3) 2_656 2_656 ?
O13 V2 Mo1 111.1(3) . 2_656 ?
O13 V2 Mo1 111.1(3) 2_656 . ?
O13 V2 Mo2 40.6(3) . . ?
O13 V2 Mo2 111.0(3) 2_656 . ?
O13 V2 Mo2 40.6(3) 2_656 2_656 ?
O13 V2 Mo2 111.0(3) . 2_656 ?
O14 V2 O13 81.1(4) . 2_656 ?
O14 V2 O13 81.1(4) 2_656 . ?
O14 V2 O13 80.9(4) 2_656 2_656 ?
O14 V2 O13 80.9(4) . . ?
O14 V2 O14 133.1(6) . 2_656 ?
O14 V2 Mo1 110.8(3) 2_656 . ?
O14 V2 Mo1 40.5(3) . . ?
O14 V2 Mo1 110.8(3) . 2_656 ?
O14 V2 Mo1 40.5(3) 2_656 2_656 ?
O14 V2 Mo2 40.4(3) . 2_656 ?
O14 V2 Mo2 110.8(3) 2_656 2_656 ?
O14 V2 Mo2 110.8(3) . . ?
O14 V2 Mo2 40.4(3) 2_656 . ?
O18 V2 O13 113.1(3) . . ?
O18 V2 O13 113.1(3) . 2_656 ?
O18 V2 O14 113.5(3) . . ?
O18 V2 O14 113.5(3) . 2_656 ?
O18 V2 Mo1 120.66(4) . 2_656 ?
O18 V2 Mo1 120.66(4) . . ?
O18 V2 Mo2 120.63(4) . 2_656 ?
O18 V2 Mo2 120.63(4) . . ?
Mo1 V2 Mo1 118.68(9) . 2_656 ?
Mo1 V2 Mo2 74.94(5) 2_656 2_656 ?
Mo1 V2 Mo2 74.94(5) . 2_656 ?
Mo1 V2 Mo2 74.94(5) . . ?
Mo1 V2 Mo2 74.94(5) 2_656 . ?
Mo2 V2 Mo2 118.73(9) 2_656 . ?
Mo2 O15 Mo6 142.0(8) . 5_656 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
C4 N7 N14 C1 -1.2(11) 8 . . 8 ?
C4 N7 N14 Co2 173.9(7) 8 . . . ?
C6 N4 N10 C5 1.6(12) . . . . ?
C6 N4 N10 Co4 -169.3(7) . . . . ?
C8 N1 N9 C2 1.1(12) . . . . ?
C8 N1 N9 Co1 -169.4(7) . . . . ?
C9 N17 N18 C12 -2.5(15) . . . . ?
C9 N17 N18 Co5 -177.9(8) . . . . ?
C10 N12 N13 C11 -1.1(14) . . . . ?
C10 N12 N13 Co2 -177.4(8) . . . . ?
N1 C8 N3 C2 0.0(13) . . . . ?
N1 C8 N3 Co3 172.5(7) . . . . ?
N2 C5 N10 N4 -1.2(13) . . . . ?
N2 C5 N10 Co4 168.6(7) . . . . ?
N2 C6 N4 N10 -1.6(13) . . . . ?
N2 C6 N4 Co5 169.8(7) . . . . ?
N3 C2 N9 N1 -1.2(13) . . . . ?
N3 C2 N9 Co1 168.0(7) . . . . ?
N3 C8 N1 N9 -0.7(12) . . . . ?
N3 C8 N1 Co2 169.6(7) . . . . ?
N4 C6 N2 C5 0.9(13) . . . . ?
N4 C6 N2 Co3 172.9(7) . . . . ?
N5 C3 N8 N11 -0.2(12) . . . 7_657 ?
N5 C3 N8 Co4 163.3(7) . . . . ?
N7 C4 N6 C1 -1.2(13) 8_455 . . . ?
N7 C4 N6 Co5 -171.4(7) 8_455 . . . ?
N8 C3 N5 C7 -0.5(12) . . . . ?
N8 C3 N5 Co2 -171.8(7) . . . . ?
N9 C2 N3 C8 0.7(13) . . . . ?
N9 C2 N3 Co3 -170.7(8) . . . . ?
N10 C5 N2 C6 0.2(12) . . . . ?
N10 C5 N2 Co3 -170.6(8) . . . . ?
N11 C7 N5 C3 1.0(12) 7_657 . . . ?
N11 C7 N5 Co2 172.9(7) 7_657 . . . ?
N12 C10 N16 C11 0.4(18) . . . . ?
N13 C11 N16 C10 -1.1(18) . . . . ?
N14 C1 N6 C4 2.1(13) 8_455 . . . ?
N14 C1 N6 Co5 172.9(7) 8_455 . . . ?
N15 C9 N17 N18 1.5(16) . . . . ?
N15 C9 N17 Co4 179.3(10) . . . . ?
N15 C12 N18 N17 2.5(17) . . . . ?
N15 C12 N18 Co5 177.0(10) . . . . ?
N16 C10 N12 N13 0.4(15) . . . . ?
N16 C10 N12 Co1 179.9(9) . . . . ?
N16 C11 N13 N12 1.3(16) . . . . ?
N16 C11 N13 Co2 177.0(10) . . . . ?
N17 C9 N15 C12 -0.1(18) . . . . ?
N18 C12 N15 C9 -1.6(19) . . . . ?
O11 Mo2 O15 Mo6 -97.6(12) . . . 5_656 ?
O12 Mo2 O15 Mo6 156.5(12) . . . 5_656 ?
O13 Mo2 O15 Mo6 3(2) . . . 5_656 ?
O14 Mo2 O15 Mo6 56.9(12) 2_656 . . 5_656 ?
O16 O16 P1 O16 180.000(5) 6_565 . . 2_656 ?
O16 O16 P1 O17 61.0(7) 6_565 . . 2_656 ?
O16 O16 P1 O17 -119.0(7) 6_565 . . 6_565 ?
O16 O16 P1 O17 -60.7(7) 6_565 . . . ?
O16 O16 P1 O17 119.3(7) 6_565 . . 5_666 ?
O16 O17 P1 O16 121.5(11) 5_666 . . 6_565 ?
O16 O17 P1 O16 -58.5(11) 5_666 . . 2_656 ?
O16 O17 P1 O16 180.000(1) 6_565 . . 2_656 ?
O16 O17 P1 O16 180.000(3) 5_666 . . . ?
O16 O17 P1 O16 -121.5(11) 6_565 . . 5_666 ?
O16 O17 P1 O16 58.5(11) 6_565 . . . ?
O16 O17 P1 O17 -60.9(7) 6_565 . . 2_656 ?
O16 O17 P1 O17 119.1(7) 6_565 . . 6_565 ?
O16 O17 P1 O17 60.6(7) 5_666 . . 2_656 ?
O16 O17 P1 O17 -119.4(7) 5_666 . . 6_565 ?
O17 O16 P1 O16 -61.0(7) 6_565 . . 2_656 ?
O17 O16 P1 O16 60.7(7) 5_666 . . 2_656 ?
O17 O16 P1 O16 119.0(7) 6_565 . . 6_565 ?
O17 O16 P1 O16 -119.3(7) 5_666 . . 6_565 ?
O17 O16 P1 O17 -121.7(11) 6_565 . . 5_666 ?
O17 O16 P1 O17 58.3(11) 6_565 . . . ?
O17 O16 P1 O17 180.002(2) 5_666 . . . ?
O17 O16 P1 O17 -58.3(11) 5_666 . . 2_656 ?
O17 O16 P1 O17 121.7(11) 5_666 . . 6_565 ?
O17 O16 P1 O17 180.000(4) 6_565 . . 2_656 ?
O17 O17 P1 O16 119.4(7) 6_565 . . 5_666 ?
O17 O17 P1 O16 60.9(7) 6_565 . . 2_656 ?
O17 O17 P1 O16 -119.1(7) 6_565 . . 6_565 ?
O17 O17 P1 O16 -60.6(7) 6_565 . . . ?
O17 O17 P1 O17 180.000(3) 6_565 . . 2_656 ?
O24 O24 P2 O24 180.000(3) 6 . . 2_656 ?
O24 O24 P2 O25 119.0(7) 6 . . 2_656 ?
O24 O24 P2 O25 -61.0(7) 6 . . 6 ?
O24 O24 P2 O25 -119.0(6) 6 . . . ?
O24 O24 P2 O25 61.0(6) 6 . . 5_656 ?
O24 Mo2 O15 Mo6 -3.1(11) 2_656 . . 5_656 ?
O25 O25 P2 O24 -61.3(7) 6 . . 5_656 ?
O25 O25 P2 O24 61.3(6) 6 . . 6 ?
O25 O25 P2 O24 -118.7(6) 6 . . 2_656 ?
O25 O25 P2 O24 118.7(7) 6 . . . ?
O25 O25 P2 O25 180.000(1) 6 . . 2_656 ?
O25 Mo2 O15 Mo6 -32.3(13) 2_656 . . 5_656 ?
Co1 N7 N14 C1 164.0(7) . . . 8 ?
Co1 N7 N14 Co2 -20.9(11) . . . . ?
Co1 N12 N13 C11 179.4(10) . . . . ?
Co1 N12 N13 Co2 3.2(12) . . . . ?
Co2 N1 N9 C2 -169.1(8) . . . . ?
Co2 N1 N9 Co1 20.3(12) . . . . ?
Co4 N17 N18 C12 179.8(10) . . . . ?
Co4 N17 N18 Co5 4.4(12) . . . . ?
Co5 N4 N10 C5 -169.8(7) . . . . ?
Co5 N4 N10 Co4 19.3(12) . . . . ?
Mo1 O24 P2 O24 62.6(7) . . . 2_656 ?
Mo1 O24 P2 O24 -117.4(7) . . . 6 ?
Mo1 O24 P2 O25 -178.5(8) . . . 6 ?
Mo1 O24 P2 O25 -56.4(10) . . . 5_656 ?
Mo1 O24 P2 O25 123.6(10) . . . . ?
Mo1 O24 P2 O25 1.5(8) . . . 2_656 ?
Mo1 O25 P2 O24 178.5(8) 2_656 . . 6 ?
Mo1 O25 P2 O24 -124.2(11) 2_656 . . . ?
Mo1 O25 P2 O24 -1.5(8) 2_656 . . 2_656 ?
Mo1 O25 P2 O24 55.8(11) 2_656 . . 5_656 ?
Mo1 O25 P2 O25 -62.9(7) 2_656 . . 2_656 ?
Mo1 O25 P2 O25 117.1(7) 2_656 . . 6 ?
Mo2 O24 P2 O24 117.4(7) 2_656 . . 6 ?
Mo2 O24 P2 O24 -62.6(7) 2_656 . . 2_656 ?
Mo2 O24 P2 O25 178.4(8) 2_656 . . 5_656 ?
Mo2 O24 P2 O25 -1.6(8) 2_656 . . . ?
Mo2 O24 P2 O25 56.3(11) 2_656 . . 6 ?
Mo2 O24 P2 O25 -123.7(11) 2_656 . . 2_656 ?
Mo2 O25 P2 O24 -55.7(10) 2_656 . . 6 ?
Mo2 O25 P2 O24 1.6(8) 2_656 . . . ?
Mo2 O25 P2 O24 -178.4(8) 2_656 . . 5_656 ?
Mo2 O25 P2 O24 124.3(10) 2_656 . . 2_656 ?
Mo2 O25 P2 O25 62.9(7) 2_656 . . 2_656 ?
Mo2 O25 P2 O25 -117.1(7) 2_656 . . 6 ?
Mo3 O16 P1 O16 117.1(7) 2_656 . . 6_565 ?
Mo3 O16 P1 O16 -62.9(7) 2_656 . . 2_656 ?
Mo3 O16 P1 O17 -123.6(11) 2_656 . . 5_666 ?
Mo3 O16 P1 O17 56.4(11) 2_656 . . . ?
Mo3 O16 P1 O17 -1.9(8) 2_656 . . 6_565 ?
Mo3 O16 P1 O17 178.1(8) 2_656 . . 2_656 ?
Mo3 O17 P1 O16 56.5(11) 5_666 . . . ?
Mo3 O17 P1 O16 178.1(8) 5_666 . . 2_656 ?
Mo3 O17 P1 O16 -1.9(8) 5_666 . . 6_565 ?
Mo3 O17 P1 O16 -123.5(11) 5_666 . . 5_666 ?
Mo3 O17 P1 O17 117.2(7) 5_666 . . 6_565 ?
Mo3 O17 P1 O17 -62.8(7) 5_666 . . 2_656 ?
Mo4 O16 P1 O16 -117.1(7) 2_656 . . 6_565 ?
Mo4 O16 P1 O16 62.9(7) 2_656 . . 2_656 ?
Mo4 O16 P1 O17 123.9(11) 2_656 . . 6_565 ?
Mo4 O16 P1 O17 -56.1(11) 2_656 . . 2_656 ?
Mo4 O16 P1 O17 -177.8(8) 2_656 . . . ?
Mo4 O16 P1 O17 2.2(8) 2_656 . . 5_666 ?
Mo4 O17 P1 O16 -177.9(8) 6_565 . . . ?
Mo4 O17 P1 O16 2.1(8) 6_565 . . 5_666 ?
Mo4 O17 P1 O16 -56.3(11) 6_565 . . 2_656 ?
Mo4 O17 P1 O16 123.7(11) 6_565 . . 6_565 ?
Mo4 O17 P1 O17 -117.2(7) 6_565 . . 6_565 ?
Mo4 O17 P1 O17 62.8(7) 6_565 . . 2_656 ?
Mo6 O8 Mo1 O10 100.3(13) . . . . ?
Mo6 O8 Mo1 O13 -1(2) . . . . ?
Mo6 O8 Mo1 O14 -54.9(13) . . . . ?
Mo6 O8 Mo1 O24 5.0(11) . . . . ?
Mo6 O8 Mo1 O25 34.4(13) . . . 2_656 ?
Mo6 O8 Mo1 O26 -154.6(12) . . . . ?
Mo6 O8 Mo1 V2 -39.9(16) . . . . ?
Mo6 O24 P2 O24 0.4(11) . . . 6 ?
Mo6 O24 P2 O24 -179.6(11) . . . 2_656 ?
Mo6 O24 P2 O25 119.4(11) . . . 2_656 ?
Mo6 O24 P2 O25 -60.6(11) . . . 6 ?
Mo6 O24 P2 O25 -118.5(11) . . . . ?
Mo6 O24 P2 O25 61.5(11) . . . 5_656 ?
Mo7 O10 Mo1 O8 -96.9(12) . . . . ?
Mo7 O10 Mo1 O13 57.6(12) . . . . ?
Mo7 O10 Mo1 O14 4(2) . . . . ?
Mo7 O10 Mo1 O24 -32.1(13) . . . . ?
Mo7 O10 Mo1 O25 -2.7(11) . . . 2_656 ?
Mo7 O10 Mo1 O26 156.8(12) . . . . ?
Mo7 O10 Mo1 V2 42.9(15) . . . . ?
Mo7 O11 Mo2 O12 -155.7(12) . . . . ?
Mo7 O11 Mo2 O13 -56.3(12) . . . . ?
Mo7 O11 Mo2 O14 -3(2) . . . 2_656 ?
Mo7 O11 Mo2 O24 33.2(13) . . . 2_656 ?
Mo7 O11 Mo2 O25 3.8(10) . . . 2_656 ?
Mo7 O11 Mo2 V2 -41.3(15) . . . . ?
Mo7 O11 Mo2 O15 98.9(12) . . . . ?
Mo7 O25 P2 O24 -118.3(10) 5_656 . . 2_656 ?
Mo7 O25 P2 O24 61.7(10) 5_656 . . 6 ?
Mo7 O25 P2 O24 119.0(10) 5_656 . . . ?
Mo7 O25 P2 O24 -61.0(10) 5_656 . . 5_656 ?
Mo7 O25 P2 O25 0.3(11) 5_656 . . 6 ?
Mo7 O25 P2 O25 -179.7(11) 5_656 . . 2_656 ?
Mo8 O3 Mo4 O2 156.6(11) 5_666 . . . ?
Mo8 O3 Mo4 O4 -96.9(12) 5_666 . . . ?
Mo8 O3 Mo4 O16 -31.6(12) 5_666 . . 2_656 ?
Mo8 O3 Mo4 O17 -2.6(10) 5_666 . . 6_565 ?
Mo8 O3 Mo4 O22 56.6(11) 5_666 . . 2_656 ?
Mo8 O3 Mo4 O23 4(2) 5_666 . . 2_656 ?
Mo8 O3 Mo4 V1 43.6(14) 5_666 . . . ?
Mo8 O5 Mo3 O16 32.8(14) . . . 2_656 ?
Mo8 O5 Mo3 O17 3.8(12) . . . 5_666 ?
Mo8 O5 Mo3 O20 98.2(14) . . . . ?
Mo8 O5 Mo3 O21 -157.0(13) . . . . ?
Mo8 O5 Mo3 O22 -55.3(14) . . . . ?
Mo8 O5 Mo3 O23 -1(2) . . . 2_656 ?
Mo8 O5 Mo3 V1 -41.6(17) . . . . ?
Mo8 O17 P1 O16 119.0(11) 5_666 . . 5_666 ?
Mo8 O17 P1 O16 -61.0(11) 5_666 . . . ?
Mo8 O17 P1 O16 -119.5(11) 5_666 . . 6_565 ?
Mo8 O17 P1 O16 60.5(11) 5_666 . . 2_656 ?
Mo8 O17 P1 O17 -0.4(12) 5_666 . . 6_565 ?
Mo8 O17 P1 O17 179.6(12) 5_666 . . 2_656 ?
Mo5 O4 Mo4 O2 -158.0(13) . . . . ?
Mo5 O4 Mo4 O3 97.8(13) . . . . ?
Mo5 O4 Mo4 O16 3.0(11) . . . 2_656 ?
Mo5 O4 Mo4 O17 32.1(14) . . . 6_565 ?
Mo5 O4 Mo4 O22 -2(2) . . . 2_656 ?
Mo5 O4 Mo4 O23 -56.3(13) . . . 2_656 ?
Mo5 O4 Mo4 V1 -42.5(16) . . . . ?
Mo5 O16 P1 O16 -0.3(12) 5_666 . . 6_565 ?
Mo5 O16 P1 O16 179.7(12) 5_666 . . 2_656 ?
Mo5 O16 P1 O17 -61.0(11) 5_666 . . . ?
Mo5 O16 P1 O17 119.0(11) 5_666 . . 5_666 ?
Mo5 O16 P1 O17 -119.3(11) 5_666 . . 6_565 ?
Mo5 O16 P1 O17 60.7(11) 5_666 . . 2_656 ?
Mo5 O20 Mo3 O5 -96.6(12) . . . . ?
Mo5 O20 Mo3 O16 -2.7(10) . . . 2_656 ?
Mo5 O20 Mo3 O17 -31.6(12) . . . 5_666 ?
Mo5 O20 Mo3 O21 156.5(11) . . . . ?
Mo5 O20 Mo3 O22 4(2) . . . . ?
Mo5 O20 Mo3 O23 56.7(11) . . . 2_656 ?
Mo5 O20 Mo3 V1 43.4(14) . . . . ?
V2 Mo2 O15 Mo6 42.3(15) . . . 5_656 ?

_olex2_submission_special_instructions 'No special instructions were received'

# SQUEEZE RESULTS (Version = 120416)
# Note: Data are Listed for all Voids in the P1 Unit Cell
# i.e. Centre of Gravity, Solvent Accessible Volume,
# Recovered number of Electrons in the Void and
# Details about the Squeezed Material
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.000 0.000 0.000 425 125 ' '
2 0.500 0.000 0.000 427 128 ' '
3 0.500 0.500 0.000 425 125 ' '
4 0.000 0.500 0.000 427 128 ' '
_platon_squeeze_void_probe_radius 1.20
_platon_squeeze_details          ?
